# cif

formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p5 Note: P = 2.66 GPa
formula_title: <missing>
a: 4.7581
b: 4.7581
c: 15.473
alpha: 90
beta: 90
gamma: 120
cell_volume: 303.370
crystal_density: 3.756
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAkGkQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: oL4AAKC+AACgjAAAgLsAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: 0J0AANCdAABwewAA
atoms_aniso_u22: 0J0AANCdAABAnAAA
atoms_aniso_u33: 0AEBANABAQCAOAEA
atoms_aniso_u12: IE4AACBOAABAUQAA
atoms_aniso_u13: AAAAAAAAAAAw+P//
atoms_aniso_u23: AAAAAAAAAABg8P//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAQAACAAAgAAAEAAACAAAACABAAAAAAAEEAAAMAIYQAAAAAQACAIAgAIBCAAMAiAAAAEQAQEgAAAiAAgREAQAEAQIAAABABgEgCCQAQSAACUAgkAAAQEEEACQBBSAgCABAA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p6 Note: P = 3.57 GPa
formula_title: <missing>
a: 4.7426
b: 4.7426
c: 15.368
alpha: 90
beta: 90
gamma: 120
cell_volume: 299.351
crystal_density: 3.806
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAIGsQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: sLMAALCzAAAgywAAIMsAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: ILIAACCyAADgqwAA
atoms_aniso_u22: ILIAACCyAADA2gAA
atoms_aniso_u33: gLsAAIC7AADA2gAA
atoms_aniso_u12: EFkAABBZAACAcAAA
atoms_aniso_u13: AAAAAAAAAACg9v//
atoms_aniso_u23: AAAAAAAAAABg8P//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAIAABAAAQAAACAAABAAAABAAQAAAAAABBAAABACCEAAAAACAAQCAIACARAABAIgAAABEAEBEAAAIgAECRACAAgCBAAAAQAIAkAQkACCQAAkQEEgAACAQggASAEKQEAQAEA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p7 Note: P = 4.39 GPa
formula_title: <missing>
a: 4.7409
b: 4.7409
c: 15.319
alpha: 90
beta: 90
gamma: 120
cell_volume: 298.183
crystal_density: 3.821
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAIGsQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: ILIAACCyAADgqwAAAK8AAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: 0J0AANCdAABQqgAA
atoms_aniso_u22: 0J0AANCdAABAnAAA
atoms_aniso_u33: wNoAAMDaAAAgywAA
atoms_aniso_u12: IE4AACBOAACQTAAA
atoms_aniso_u13: AAAAAAAAAADw8f//
atoms_aniso_u23: AAAAAAAAAABw5f//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAIAAAgAAQAAACAAABAAAABAAIAAAAAABBAAABgBCEAAAAACAAIBAIACAQgAAgIQAAAAiACAiAAAIgAEBJACAAgBBAAAAIAMAUAQSABDQAASQCEQAABAIQgAKAEFQEAIAEA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p8 Note: P = 4.74 GPa
formula_title: <missing>
a: 4.7415
b: 4.7415
c: 15.308
alpha: 90
beta: 90
gamma: 120
cell_volume: 298.044
crystal_density: 3.823
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAEHYQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: oL4AAKC+AABg6gAAgLsAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: 4MQAAODEAACgjAAA
atoms_aniso_u22: 4MQAAODEAACgjAAA
atoms_aniso_u33: 4KsAAOCrAACgCQEA
atoms_aniso_u12: cGIAAHBiAACAPgAA
atoms_aniso_u13: AAAAAAAAAACg9v//
atoms_aniso_u23: AAAAAAAAAABg8P//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAIAAAgAAQAAACAAABAAAABAAIAAAAAABBAAABgBDEAAAAACAAIBAIACAQgAAwIQAAAAiACAiAAAIgAEBJACAAgBBAAAAIAMAUAQSACDQAASQCEQAABAIQgAKAEFQEAIAEA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p9 Note: P = 5.20 GPa
formula_title: <missing>
a: 4.7388
b: 4.7388
c: 15.287
alpha: 90
beta: 90
gamma: 120
cell_volume: 297.296
crystal_density: 3.832
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAwGEQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: MNkAADDZAACAuwAAwNoAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: 0M8AANDPAADgqwAA
atoms_aniso_u22: 0M8AANDPAABAnAAA
atoms_aniso_u33: 8OsAAPDrAADAVwEA
atoms_aniso_u12: IGcAACBnAABAUQAA
atoms_aniso_u13: AAAAAAAAAABgCQAA
atoms_aniso_u23: AAAAAAAAAACgDwAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAEAAAQAAQAAACAAABAAAABAAMAAAAAABBAAABQBDEAAAAABAAIBgIABAIgAAwEQAAAAhACASAAAEgAGBIgCAAQBAgAAAIAGASAQSABBIAASQDCQAAAgEQQAJAGEoCAEAEA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p10 Note: P = 6.33 GPa
formula_title: <missing>
a: 4.7332
b: 4.7332
c: 15.1926
alpha: 90
beta: 90
gamma: 120
cell_volume: 294.763
crystal_density: 3.865
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAUHwQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: YNEAAGDRAACgjAAAIMsAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: QAABAEAAAQAgywAA
atoms_aniso_u22: QAABAEAAAQDAXQAA
atoms_aniso_u33: AH0AAAB9AACgCQEA
atoms_aniso_u12: IIAAACCAAADgLgAA
atoms_aniso_u13: AAAAAAAAAAAA5///
atoms_aniso_u23: AAAAAAAAAAAg0f//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAACAAAIAAQAAABAAAAgAAAAgAFAAAAAAAggAAAkARSAAAAAAgABAQEABAIQAAUCIAAAAQgBAIgAACQACgUgBAAIAQYAAAEACgGAIIgAg0AAEkAwsAAAICCIACgBiUAgBABA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p11 Note: P = 7.01 GPa
formula_title: <missing>
a: 4.7248
b: 4.7248
c: 15.1242
alpha: 90
beta: 90
gamma: 120
cell_volume: 292.395
crystal_density: 3.897
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAUHwQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: ILIAACCyAADQhAAAEL0AAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: 4JIAAOCSAACQlwAA
atoms_aniso_u22: 4JIAAOCSAAAgywAA
atoms_aniso_u33: MPIAADDyAABg6gAA
atoms_aniso_u12: cEkAAHBJAAAgZwAA
atoms_aniso_u13: AAAAAAAAAAAAAAAA
atoms_aniso_u23: AAAAAAAAAABw/v//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAACAAAEAAIAAAAgAAAgAAAAQACgAAAAAAgQAAARAIlAAAAAAIAAQMCAAgEIAAJBEAAAAIQAgCIAABEAAoJIAgACAEMAAACAAoBgCEgAIOAACRAULAAAEAhEABQAkVAQAgAQ==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p12 Note: P = 8.33 GPa
formula_title: <missing>
a: 4.7177
b: 4.7177
c: 15.043
alpha: 90
beta: 90
gamma: 120
cell_volume: 289.952
crystal_density: 3.929
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAsIUQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: YLgAAGC4AABwlAAAUMMAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: EKQAABCkAADAqAAA
atoms_aniso_u22: EKQAABCkAAAgywAA
atoms_aniso_u33: AOEAAADhAADA2gAA
atoms_aniso_u12: QFEAAEBRAACQZQAA
atoms_aniso_u13: AAAAAAAAAACw6///
atoms_aniso_u23: AAAAAAAAAABg1///
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAABAAABAAIAAAAgAAAQAAAAIAAoAAAAAAQQAAAIQCRAAAAAAEAAEFBAAQCEAAEQRAAAAEEAQBCAABEAASCkAIABABDAAABAASAQBBIAIGgABIQFDQAABAERAAUAKJgEAIAM==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p13 Note: P = 9.17 GPa
formula_title: <missing>
a: 4.7146
b: 4.7146
c: 14.9903
alpha: 90
beta: 90
gamma: 120
cell_volume: 288.556
crystal_density: 3.948
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAEI8QAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: 8LkAAPC5AAAgywAAYOoAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: UJEAAFCRAACgCQEA
atoms_aniso_u22: UJEAAFCRAAAA+gAA
atoms_aniso_u33: oAkBAKAJAQDgqwAA
atoms_aniso_u12: 4EcAAOBHAABwewAA
atoms_aniso_u13: AAAAAAAAAABQyf//
atoms_aniso_u23: AAAAAAAAAACgkv//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAgAAAgAEAAAAQAAAQAAAAIAAkAAAAAAQIAAAIIBIgAAAAACAACDBAAICEAACIRAAAAECAIAhAAAiAARBUAIAAgARgAAAgARAIBAkAEDQAAkIESoAABACJAASAElQCAEAD==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p14 Note: P = 9.82 GPa
formula_title: <missing>
a: 4.7087
b: 4.7087
c: 14.9313
alpha: 90
beta: 90
gamma: 120
cell_volume: 286.702
crystal_density: 3.974
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAwJMQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: 8NIAAPDSAAAAlgAA4N0AAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: kMkAAJDJAABwxgAA
atoms_aniso_u22: kMkAAJDJAAAA+gAA
atoms_aniso_u33: QOcAAEDnAABg6gAA
atoms_aniso_u12: AGQAAABkAAAggAAA
atoms_aniso_u13: AAAAAAAAAACg3f//
atoms_aniso_u23: AAAAAAAAAABAu///
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAgAAAQAEAAAAQAAAIAAAAEAASAAAAAAIIAAAECAkwAAAAABAABBQgAIBCAACCEgAAACBAEAIgAARAAEQqAEAAQAIwAAAQAEQGAgiABA4AASECIqAAAQBCgAJACRYCABAB==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p15 Note: P = 10.88 GPa
formula_title: <missing>
a: 4.7017
b: 4.7017
c: 14.855
alpha: 90
beta: 90
gamma: 120
cell_volume: 284.389
crystal_density: 4.006
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAIIQQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: gKIAAICiAADwhwAA4MQAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: QJwAAECcAAAQiwAA
atoms_aniso_u22: QJwAAECcAAAgywAA
atoms_aniso_u33: kLAAAJCwAABAGQEA
atoms_aniso_u12: IE4AACBOAABwYgAA
atoms_aniso_u13: AAAAAAAAAADg4///
atoms_aniso_u23: AAAAAAAAAAAwxv//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAQAAAIAEAAAAIAAAIAAAACAAEgAAAAAEEAAACAgKUAAAAAAgAAQogAEAhAAAgiQAAABAgCAEIAAIgACENACAAEACUAAAIACEDAIJAAgaAAJBAiNAAAEAJIACgAisAgAgA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p16 Note: P = 11.90 GPa
formula_title: <missing>
a: 4.6955
b: 4.6955
c: 14.7918
alpha: 90
beta: 90
gamma: 120
cell_volume: 282.433
crystal_density: 4.034
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAkIIQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: YLgAAGC4AACAiQAAUMMAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: 8KAAAPCgAACAiQAA
atoms_aniso_u22: 8KAAAPCgAACAuwAA
atoms_aniso_u33: IOQAACDkAABAGQEA
atoms_aniso_u12: QFEAAEBRAAAwXAAA
atoms_aniso_u13: AAAAAAAAAAAA5///
atoms_aniso_u23: AAAAAAAAAAAAzv//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAIAAAEACAAAAIAAAEAAAABAACQAAAAAECAAABAIFJAAAAAAQAAESQACAQgAAgRIAAAAgIBABCAAEQABCGgAgACAAmAAAEABCBQEEgAQLAACQgQmQAACAEUABIARNAQAIA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p17 Note: P = 12.73 GPa
formula_title: <missing>
a: 4.6929
b: 4.6929
c: 14.7382
alpha: 90
beta: 90
gamma: 120
cell_volume: 281.098
crystal_density: 4.053
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAYHEQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: UMMAAFDDAACgjAAAwNoAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: cMYAAHDGAADw6wAA
atoms_aniso_u22: cMYAAHDGAACgCQEA
atoms_aniso_u33: gLsAAIC7AABAnAAA
atoms_aniso_u12: AGQAAABkAADQhAAA
atoms_aniso_u13: AAAAAAAAAACwBAAA
atoms_aniso_u23: AAAAAAAAAACgDwAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAIAAACACAAAAEAAAEAAAABAACIAAAAAECAAABACDIgAAAAAIAABKIABAQgAAQFEAAAAgIBAAhAAEQABAjQAgABAAVAAACABBBQECQAIFAACQQQTEAABABMABEAQagIAEA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p18 Note: P = 14.82 GPa
formula_title: <missing>
a: 4.6826
b: 4.6826
c: 14.613
alpha: 90
beta: 90
gamma: 120
cell_volume: 277.488
crystal_density: 4.106
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAQIcQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: ILIAACCyAAAQpAAAkMkAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: AJYAAACWAACQfgAA
atoms_aniso_u22: AJYAAACWAABAnAAA
atoms_aniso_u33: 0OgAANDoAAAgSAEA
atoms_aniso_u12: AEsAAABLAABAUQAA
atoms_aniso_u13: AAAAAAAAAADw8f//
atoms_aniso_u23: AAAAAAAAAADg4///
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAEAAAAgCAAAACAAACAAAAAgAAhAAAAACBAAAAQAQUEAAAAABAAAKUAAgIQAAIAqAAAAICAQAIIABEAAQEYAQAAQADIAABAAIERAhIAEBIAAkECCRAAAQAJgAKACDoCABA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p19 Note: P = 16.42 GPa
formula_title: <missing>
a: 4.6775
b: 4.6775
c: 14.528
alpha: 90
beta: 90
gamma: 120
cell_volume: 275.273
crystal_density: 4.139
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAgHQQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: 4N0AAODdAACAuwAAYOoAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: AOEAAADhAACgjAAA
atoms_aniso_u22: AOEAAADhAABAGQEA
atoms_aniso_u33: wNoAAMDaAAAgSAEA
atoms_aniso_u12: gHAAAIBwAACgjAAA
atoms_aniso_u13: AAAAAAAAAABw/v//
atoms_aniso_u23: AAAAAAAAAAAAAAAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAACAAAAIBAAAACAAACAAAAAQAAQQAAAACAgAAAQAEMBAAAAAAgAADEAAQEIAACAMgAAAEAgIACCABCAAIBMAEAAEAA0AAAgAECIggkABAcAASBCAkQAAEAEgAEgBAsBAAQ==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p20 Note: P = 17.66 GPa
formula_title: <missing>
a: 4.6679
b: 4.6679
c: 14.4441
alpha: 90
beta: 90
gamma: 120
cell_volume: 272.561
crystal_density: 4.180
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAA8HIQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: cEMBAHBDAQBg6gAAIEgBAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: YBwBAGAcAQDA2gAA
atoms_aniso_u22: YBwBAGAcAQAA+gAA
atoms_aniso_u33: QJYBAECWAQCgAwIA
atoms_aniso_u12: MI4AADCOAAAAfQAA
atoms_aniso_u13: AAAAAAAAAADgFQAA
atoms_aniso_u23: AAAAAAAAAADgLgAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAABAAAAEBAAAABAAABAAAAAIAAEEAAAAAggAAAIAAnAQAAAAAIAAAzAAICEAABACQAAACAICAAggARAACASACAABAAEgAAIACASIIRAAQJgAIgQQHCAABAAkACQAQGAIAE==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p21 Note: P = 18.69 GPa
formula_title: <missing>
a: 4.6686
b: 4.6686
c: 14.401
alpha: 90
beta: 90
gamma: 120
cell_volume: 271.829
crystal_density: 4.191
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAoKkQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: 4EEBAOBBAQAAdwEAIEgBAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: MAsBADALAQAgSAEA
atoms_aniso_u22: MAsBADALAQDgqwAA
atoms_aniso_u33: gLUBAIC1AQCAtQEA
atoms_aniso_u12: 0IQAANCEAAAgTgAA
atoms_aniso_u13: AAAAAAAAAABAHwAA
atoms_aniso_u23: AAAAAAAAAACAPgAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAAgAAACBAAAABAAABAAAAAIAAECAAAABAgAAAIAATAIAAAAAIAAAbAAICEAABACwAAACAICAAggARAACALACAABAAEgAAIACASEIRAAQFgAIgQQHCAABAAUACQAQGAQAC==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p22 Note: P = 19.78 GPa
formula_title: <missing>
a: 4.6641
b: 4.6641
c: 14.341
alpha: 90
beta: 90
gamma: 120
cell_volume: 270.175
crystal_density: 4.217
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAMKsQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: YLgAAGC4AACgjAAA4KsAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: AK8AAACvAABwxgAA
atoms_aniso_u22: AK8AAACvAABAGQEA
atoms_aniso_u33: IMsAACDLAAAgTgAA
atoms_aniso_u12: gFcAAIBXAACAiQAA
atoms_aniso_u13: AAAAAAAAAADg/P//
atoms_aniso_u23: AAAAAAAAAAAAAAAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAgAAABBAAAAAgAABAAAAAEAACBAAAAAgQAAAEAAHQCAAAAAEAAANQAECCAABAA4AAABAECAAQIAQgACADgBAAAgADQAAEABAFBEIgAQCwAEgIIBxAAAQAGABIAIDAIAB==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p23 Note: P = 20.24 GPa
formula_title: <missing>
a: 4.6624
b: 4.6624
c: 14.330
alpha: 90
beta: 90
gamma: 120
cell_volume: 269.771
crystal_density: 4.223
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAgKYQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: wKgAAMCoAABAgwAAoKUAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: kJcAAJCXAADgqwAA
atoms_aniso_u22: kJcAAJCXAABg6gAA
atoms_aniso_u33: kMkAAJDJAABgbQAA
atoms_aniso_u12: AEsAAABLAAAQcgAA
atoms_aniso_u13: AAAAAAAAAAAAAAAA
atoms_aniso_u23: AAAAAAAAAACQAQAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAgAAABAgAAAAgAABAAAAAEAABAgAAAAgQAAACAAHQCAAAAACAAANQAEBCAAAgAoAAABAEBAAIIAIgABADgBAAAQADIAAEAAgDBCIgAICwAEQEIBwgAAIAGAAkAIDgIAB==


formula: Mn Sn (O6 H6)
compound: Synthetic
pub_title: Hydrothermal preparation of hydroxy stannates. The crystal structure of MnSn(OH)6
formula_title: <missing>
a: 7.885
b: 7.885
c: 7.885
alpha: 90
beta: 90
gamma: 90
cell_volume: 490.236
crystal_density: 3.735
atoms_sites: ["Mn", "Sn", "O-H"]
atoms_x: AAAAAICEHgCg8QQA
atoms_y: AAAAAICEHgBAwzgA
atoms_z: AAAAAICEHgBgkA8A
atoms_occupancy: 0
atoms_u_iso: SKgAAAhhAACwOgEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAABAAAAAAAEAAAAAEAAAAEAAAAgAAAgAACAAAQAAIAAIAAIAAgACAAAACAAQAIACABAAgAgAQAQAgBABACAIAQAAEAQBAEAQCAIBAIBAQCAQCAgABAQEBAQICAgIABAQIECAAQIECBBAgQQIIACBBA==


formula: (Mg1.8 Fe.2) Si O4
compound: Baldissero, Ivrea-Verbano Zone, Western Italian Alps
formula_title: <missing>
a: 4.759
b: 10.227
c: 5.995
alpha: 90
beta: 90
gamma: 90
cell_volume: 291.778
crystal_density: 3.346
atoms_sites: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAwYv//MGL//8AMGgDAwC4AwBARAAD+EAA=
atoms_y: AAAAAAAAAAAA9BAAAPQQABDCBQDQmAUAIMr8/9D4CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAMAGAgA=
atoms_occupancy: oL82AGBJBgBgHTcAoOsFAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: EEAAABBAAACwTwAAsE8AAGAiAAAwKgAA4EcAAABLAAA=
atoms_aniso_u22: sIEAALCBAABAUQAAQFEAALBPAABwewAAIE4AAIBwAAA=
atoms_aniso_u33: cGIAAHBiAAAQcgAAEHIAABBZAABAagAAIIAAALBoAAA=
atoms_aniso_u12: 4Pz//+D8//9w/v//cP7//wAAAACADAAAsAQAACADAAA=
atoms_aniso_u13: wPn//8D5//8AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: 0O7//9Du//8AAAAAAAAAAAAAAAAAAAAAAAAAAMASAAA=
pub_title:
 Crystal chemistry of the olivines in the peridotites from the Ivrea-
 Verbano Zone (Western Italian Alps)
 Note: Sample Mo895

qdat:
AAAAAAAAAAAAAAAAAAAAUAAAAAAAQBAAAABoAAAAEqEAgQQIECAGALQAVSYBaECAiBAEM3iMBRjqkkAHChGa5dCAzqun8zDSbxK+hxc8NAz+6trNNu/VNfCGxXO173Z6nQvV275k/xcu1Pv2VtfL3Prou7f5YGrf7+j8n/==


formula: (Mg1.8 Fe.2) Si O4
compound: Balmuccia, Ivrea-Verbano Zone, Western Italian Alps
formula_title: <missing>
a: 4.764
b: 10.226
c: 5.991
alpha: 90
beta: 90
gamma: 90
cell_volume: 291.862
crystal_density: 3.345
atoms_sites: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABQZf//UGX//1AOGgCAui4AwBARAHD8EAA=
atoms_y: AAAAAAAAAADo8hAA6PIQABDCBQDQmAUA0M78//j4CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAMAGAgA=
atoms_occupancy: IP42AOAKBgDg3jYAICoGAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: UJEAAFCRAABwrQAAcK0AADB1AADgeQAAYJ8AAOCSAAA=
atoms_aniso_u22: sIEAALCBAABQXwAAUF8AAEBRAACgcwAAkEwAAAB9AAA=
atoms_aniso_u33: oIwAAKCMAAAgmQAAIJkAAECDAACwmgAAwKgAAHCUAAA=
atoms_aniso_u12: kAEAAJABAACQAQAAkAEAACADAADQBwAAIAMAAEAGAAA=
atoms_aniso_u13: EPX//xD1//8AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: IOr//yDq//8AAAAAAAAAAAAAAAAAAAAAAAAAAMASAAA=
pub_title:
 Crystal chemistry of the olivines in the peridotites from the Ivrea-
 Verbano Zone (Western Italian Alps)
 Note: Sample 77IVBL11

qdat:
AAAAAAAAAAAAAAAAAAAAMAAAAAAAgBAAAABoAAAAEqEAgQQIMCAEAHQAZRYBVEEAiBAEU2iUBJjs0sAFChCSxdCA1qen2zDSbxc+hpt+NAza69rNN63dN1CKxPd1r366lQvXa/fpvR6/9Pt+l+er3X3w67fw4Lz9b9X/n3==


formula: (Mg1.828 Fe.172) Si O4
compound: Finero, Ivrea-Verbano Zone, Western Italian Alps
formula_title: <missing>
a: 4.762
b: 10.231
c: 5.993
alpha: 90
beta: 90
gamma: 90
cell_volume: 291.979
crystal_density: 3.324
atoms_sites: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAD4Yv//+GL//+AKGgBQwi4AoA0RAHD8EAA=
atoms_y: AAAAAAAAAADQ8RAA0PEQAMDBBQBAlwUAKMz8/2j3CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPADAFAgA=
atoms_occupancy: AKo3AABfBQCA6DcAgCAFAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: YFQAAGBUAADQawAA0GsAAGA7AACAPgAAMFwAAMBdAAA=
atoms_aniso_u22: oFoAAKBaAAAgNQAAIDUAAFAtAAAQWQAAkDMAANBSAAA=
atoms_aniso_u33: EFkAABBZAAAAZAAAAGQAACBOAAAAZAAAYG0AAHBiAAA=
atoms_aniso_u12: AAAAAAAAAAAgAwAA4Pz//1gCAADA+f//cP7//7AEAAA=
atoms_aniso_u13: EPX//xD1//8AAAAAAAAAAAAAAAAAAAAAAAAAAFD7//8=
atoms_aniso_u23: kO3//5Dt//8AAAAAAAAAAAAAAAAAAAAAAAAAAHAXAAA=
pub_title:
 Crystal chemistry of the olivines in the peridotites from the Ivrea-
 Verbano Zone (Western Italian Alps)
 Note: Sample PB9

qdat:
AAAAAAAAAAAAAAAAAAAAUAAAAAAAQBAAAABoAAAAEqEAgQQIMCAEAHgAZSYBaEEAiBAEU2iUBRjs0sAFChGSxZCA1qen8yDSbxc+hxs+NA3batrNN23dP3GLRXO3r3y+lQvV+/7JvQ6/9Nt2lvfL3P3w27f44Pz9b/j+n/==


formula: (Mg1.774 Fe.226) Si O4
compound: Rocca d'Argimonia, Ivrea-Verbano Zone, Western Italian Alps
formula_title: <missing>
a: 4.762
b: 10.230
c: 5.996
alpha: 90
beta: 90
gamma: 90
cell_volume: 292.097
crystal_density: 3.361
atoms_sites: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAA4X///OF///xgKGgDgwy4AwBARAAD+EAA=
atoms_y: AAAAAAAAAABg8xAAYPMQAKDDBQCwlQUAmM/8/+D3CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPADAFAgA=
atoms_occupancy: IAQ2AOAEBwCgQjYAYMYGAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: QFEAAEBRAABAUQAAQFEAACA1AADwPAAA0FIAAIBXAAA=
atoms_aniso_u22: AH0AAAB9AABgVAAAYFQAAEBRAAAggAAAEFkAAFB4AAA=
atoms_aniso_u33: 8FUAAPBVAACgWgAAoFoAAOBHAADgYAAAAGQAAMBdAAA=
atoms_aniso_u12: AAAAAAAAAACQAQAAkAEAAJABAAAAAAAAsAQAACADAAA=
atoms_aniso_u13: EPX//xD1//8AAAAAAAAAAAAAAAAAAAAAAAAAAFD7//8=
atoms_aniso_u23: QO3//0Dt//8AAAAAAAAAAAAAAAAAAAAAAAAAAAAZAAA=
pub_title:
 Crystal chemistry of the olivines in the peridotites from the Ivrea-
 Verbano Zone (Western Italian Alps)
 Note: Sample Mo982

qdat:
AAAAAAAAAAAAAAAAAAAAUAAAAAAAgBAAAABoAAAAEqEAgQgIMCAEALgAZSYBaEEAkBAEU3iUBRjsksAFChGSx5CB2q+n8yDUbxd/BxtcVA3fbtLJN23dP2GNRXe373y+lQvV897p/R8/5Pt+lNfL3P7Y2/f5QPz173n9m/==


formula: (Mg1.762 Fe.238) Si O4
compound: Finero, Ivrea-Verbano Zone, Western Italian Alps
formula_title: <missing>
a: 4.766
b: 10.236
c: 5.999
alpha: 90
beta: 90
gamma: 90
cell_volume: 292.660
crystal_density: 3.364
atoms_sites: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADwW///8Fv//6AJGgCAui4AEAwRACABEQA=
atoms_y: AAAAAAAAAAAo9BAAKPQQACjDBQDQmAUAIMr8/5D3CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPADAFAgA=
atoms_occupancy: QNU1AMAzBwAAtjUAAFMHAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: 8DwAAPA8AACwTwAAsE8AAFAUAACQGgAAIE4AADBDAAA=
atoms_aniso_u22: oIwAAKCMAAAAZAAAAGQAAHBiAAAQiwAAkDMAACCAAAA=
atoms_aniso_u33: 8DwAAPA8AABwSQAAcEkAAEA4AADwVQAAsE8AAKBBAAA=
atoms_aniso_u12: 4Pz//+D8//8AAAAAAAAAACADAAAAAAAAcP7//7AEAAA=
atoms_aniso_u13: gPP//4Dz//8AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: YPD//2Dw//8AAAAAAAAAAAAAAAAAAAAAAAAAAHAXAAA=
pub_title:
 Crystal chemistry of the olivines in the peridotites from the Ivrea-
 Verbano Zone (Western Italian Alps)
 Note: Sample 84AT7

qdat:
AAAAAAAAAAAAAAAAAAAAUAAAAAAAgBAAAACoAAAAEyEAgQgIMCAEALgAZiYCqIEAkCAEY3iYBTjtlMAOChGTx5GBms0r9yGU2iV7BSp8ZAn1z5eKXa+tbqGNTefvftzvtRel8/1K+T9/6fX7LW+Xuftxr3/ywXn937H7N/==


formula: (Mg1.684 Fe.316) Si O4
compound: Valsesia, Ivrea-Verbano Zone, Western Italian Alps
formula_title: <missing>
a: 4.765
b: 10.245
c: 6.001
alpha: 90
beta: 90
gamma: 90
cell_volume: 292.953
crystal_density: 3.416
atoms_sites: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAgVP//IFT//8AMGgBwxS4A8CERAGAHEQA=
atoms_y: AAAAAAAAAAAY9RAAGPUQAOjGBQBgmgUAgNP8/wD7CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAHALAgA=
atoms_occupancy: IJMzAOB1CQBgNTMAoNMJAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: wF0AAMBdAAAwdQAAMHUAAOBHAABAUQAAEHIAACBnAAA=
atoms_aniso_u22: 4GAAAOBgAACwNgAAsDYAAHAwAADwbgAAsDYAAKBaAAA=
atoms_aniso_u33: AEsAAABLAACwTwAAsE8AAMBEAABQXwAAgFcAAFBfAAA=
atoms_aniso_u12: cP7//3D+//8AAAAAAAAAAHD+//9w/v//kAEAACADAAA=
atoms_aniso_u13: EPX//xD1//8AAAAAAAAAAAAAAAAAAAAAAAAAAJABAAA=
atoms_aniso_u23: 0O7//9Du//8AAAAAAAAAAAAAAAAAAAAAAAAAAHAXAAA=
pub_title:
 Crystal chemistry of the olivines in the peridotites from the Ivrea-
 Verbano Zone (Western Italian Alps)
 Note: Sample Mo454

qdat:
AAAAAAAAAAAAAAAAAAAAUAAAAAAAgBAAAADIAAAAFUEAgQgIMEAMAOgAZioCqIEAkCAMY3kYCTDtpMAOChGTx6GBmu0rtSG02iV9BS58aBn2j5eKbe+ta+GOiaftfvV/uhat9/zK/T596f37KW+Xcfvjvb/ywXn53vP7N/==


formula: (Mg1.636 Fe.364) Si O4
compound: Valsesia, Ivrea-Verbano Zone, Western Italian Alps
formula_title: <missing>
a: 4.770
b: 10.253
c: 6.006
alpha: 90
beta: 90
gamma: 90
cell_volume: 293.734
crystal_density: 3.441
atoms_sites: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABAV///QFf//7AXGgBQwi4AsBsRAKANEQA=
atoms_y: AAAAAAAAAADo9xAA6PcQANjHBQCwlQUAENX8/7D6CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAHALAgA=
atoms_occupancy: AM4xAAA7CwCADDIAgPwKAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: UF8AAFBfAACgcwAAoHMAADBDAAAgTgAAgHAAAKBzAAA=
atoms_aniso_u22: oHMAAKBzAABQRgAAUEYAADBDAADQawAAYDsAAHBiAAA=
atoms_aniso_u33: 0FIAANBSAADQUgAA0FIAADBDAADQUgAAcGIAACBOAAA=
atoms_aniso_u12: IAMAACADAAAgAwAAIAMAAJABAACgDwAA0AcAALAEAAA=
atoms_aniso_u13: 8PH///Dx//8AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: 8PH///Dx//8AAAAAAAAAAAAAAAAAAAAAAAAAACAcAAA=
pub_title:
 Crystal chemistry of the olivines in the peridotites from the Ivrea-
 Verbano Zone (Western Italian Alps)
 Note: Sample Mo940

qdat:
AAAAAAAAAAAAAAAAAAAAUAAAAAAAgBAAAADIAAAAFUEBAQgQMEAMAOgAqioCqIEBECAIZqkYCVHZJIAMDCElT6MBrVdP5kOpXi9eClaoyBvenTaSf1tavsMam29f6rnfMi/bbreN+l730+v2Mt+v8bbH+r+jguvzu6fed7==


formula: (Mg1.682 Fe.318) Si O4
compound: Valsesia, Ivrea-Verbano Zone, Western Italian Alps
formula_title: <missing>
a: 4.764
b: 10.240
c: 6.002
alpha: 90
beta: 90
gamma: 90
cell_volume: 292.798
crystal_density: 3.419
atoms_sites: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACwVf//sFX//zgSGgDAwC4AIBoRAEAEEQA=
atoms_y: AAAAAAAAAAAY9RAAGPUQAOjGBQDQmAUA8NH8/2D6CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAJAOAgA=
atoms_occupancy: YDUzAKDTCQDgczMAIJUJAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: IE4AACBOAACwaAAAsGgAANA5AACgQQAAwF0AANBSAAA=
atoms_aniso_u22: MHUAADB1AADQUgAA0FIAAABLAACgcwAAcEkAAPBuAAA=
atoms_aniso_u33: 0DkAANA5AADgRwAA4EcAAEA4AABwSQAAoFoAALBPAAA=
atoms_aniso_u12: oPb//6D2//8AAAAAAAAAACADAABABgAAEA4AANAHAAA=
atoms_aniso_u13: oPb//6D2//8AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: QO3//0Dt//8AAAAAAAAAAAAAAAAAAAAAAAAAAHAXAAA=
pub_title:
 Crystal chemistry of the olivines in the peridotites from the Ivrea-
 Verbano Zone (Western Italian Alps)
 Note: Sample OLBC2

qdat:
AAAAAAAAAAAAAAAAAAAAUAAAAAAAgBAAAADIAAAAE0EAgQgIMCAMALgAZioCqIEAkCAEY3kYCTjtlMAOChGTx5GBmu8rtSG03iV3BSp8aBn1z5eJbe+ta+GNSafvfvVvmhept/zK/TZ95/+7OW+X+fvzvb/ywXn93vPrN/==


formula: (Mg1.7 Fe.3) Si O4
compound: Valsesia, Ivrea-Verbano Zone, Western Italian Alps
formula_title: <missing>
a: 4.766
b: 10.250
c: 6.005
alpha: 90
beta: 90
gamma: 90
cell_volume: 293.353
crystal_density: 3.400
atoms_sites: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACwVf//sFX//5AUGgCAui4AYCARAPAIEQA=
atoms_y: AAAAAAAAAAAI9hAACPYQACDGBQDQmAUAENX8/yD5CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAHALAgA=
atoms_occupancy: AEUzAADECQCAfTQAgIsIAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["Mg1", "Fe1", "Mg2", "Fe2", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: wCsAAMArAADQOQAA0DkAAMASAAAQJwAAcDAAAEA4AAA=
atoms_aniso_u22: YIYAAGCGAADgRwAA4EcAABBZAAAQiwAA8FUAAFB4AAA=
atoms_aniso_u33: 8G4AAPBuAAAQWQAAEFkAAMBdAAAAZAAAoIwAAFB4AAA=
atoms_aniso_u12: AAAAAAAAAAAgAwAA4Pz//wAAAACgDwAAgAwAACADAAA=
atoms_aniso_u13: cP7//3D+//8AAAAAAAAAAAAAAAAAAAAAAAAAAKD2//8=
atoms_aniso_u23: 0O7//9Du//8AAAAAAAAAAAAAAAAAAAAAAAAAAJAaAAA=
pub_title:
 Crystal chemistry of the olivines in the peridotites from the Ivrea-
 Verbano Zone (Western Italian Alps)
 Note: Sample OLBC3

qdat:
AAAAAAAAAAAAAAAAAAAAUAAAAAAAgBAAAADIAAAAFUEAgQgIMEAMAOgAaioCqIEAkCAIYqkYCTHNJIAODCElx6KBnVdP1WO02iVeDjb4aBnWjbaafdvavsMKiudf3v2/Ohe76v3K+l73S9//OtWrcW9j/f/jQfv7+2N7fd==


formula: Al2.455 Si.63 Mg.79 Na.33 O6
compound: Synthetic
formula_title: Na.41[Na.125Mg.79Al.085]2[Al.79Si.21]6O12
a: 8.7225
b: 8.7225
c: 2.7664
alpha: 90
beta: 90
gamma: 120
cell_volume: 182.275
crystal_density: 3.766
atoms_sites: ["Al1", "Si1", "Mg2", "Al2", "Na2", "Na3", "O1", "O2"]
atoms_x: UGQ8AFBkPACrsCgAq7AoAKuwKAAAAAAAsNQHAEAREwA=
atoms_y: qPcUAKj3FABVWBQAVVgUAFVYFAAAAAAA0I0kAPBYDAA=
atoms_z: QEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwA=
atoms_occupancy: wDcwAEDRDADANzAAIDAFACChBwAggwwAAAk9AAAJPQA=
atoms_u_iso: WFcAAFhXAABQkQAAUJEAAFCRAACgbgUAoIwAABCLAAA=
atoms_aniso_label: ["Al1", "Si1", "Mg2", "Al2", "Na2", "Na3", "O1", "O2"]
atoms_aniso_u11: oFoAAKBaAABQkQAAUJEAAFCRAABgbQAA0GsAABCLAAA=
atoms_aniso_u22: EFkAABBZAABQkQAAUJEAAFCRAABgbQAAYG0AAICJAAA=
atoms_aniso_u33: 0FIAANBSAADgkgAA4JIAAOCSAABAQg8AUMMAAECcAAA=
atoms_aniso_u12: UC0AAFAtAADQSAAA0EgAANBIAACwNgAAUC0AANBSAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
pub_title:
 Hexagonal Na0.41[Na0.125Mg0.79Al0.085]2[Al0.79Si0.21]6O12 (NAL phase):
 Crystal structure refinement and elasticity

qdat:
AAAAAAAAAAAAABAAAAAAAAAAgAACAAAAAAAACAAAICAABABAgAgACAAEQAAAIQCEAAAQAIAIgIgCAwAkCIEQYAqAACDIEBEAhgFAgACIWIBAYAhIEMKgowMKhgIYaJKgDQYAUiUQGMCgDKlCjGyBCqhMoLGBRkjlFQho8R==


formula: Fe Cr2 O4
compound: Synthetic
formula_title: FeCr2O4
a: 9.0633
b: 2.95793
c: 10.6391
alpha: 90
beta: 90
gamma: 90
cell_volume: 285.219
crystal_density: 5.213
atoms_sites: ["Fe1", "Cr1", "Cr2", "O1", "O2", "O3", "O4"]
atoms_x: AKAPAHAeAwCAhAUAMNESAPDFFwCQWRsAsOYEAA==
atoms_y: QEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAA==
atoms_z: QCQUAECfJQDg8QUAYFAJAPALHQCAsysAsGIaAA==
atoms_occupancy: 0
atoms_u_iso: EFMBAABkAADQUgAAMKcAADCnAAAwpwAAMKcAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure phase transitions in FeCr2O4 and structure analysis of new post-
 spinel FeCr2O4 and Fe2Cr2O5 phases with meteoritical and petrological implications

qdat:
AAAAAAAAAAAAAAAQAAACAABQAQAAAAICAAAAhEEJAgYIAGSMAAUEEIZAADSgSmAIBIAEEJtAqFM5Q3OFZ1SqVwxwRN0s18G4yjU210AZvT2Yr6fe3L8/r3cO/dvGOnX6qT0RTpd9igL/TSc1Zf+9H5onmJyzDKxTeZkLsR==


formula: Fe Cr2 O4
compound: Synthetic
formula_title: <missing>
a: 2.88445
b: 9.5207
c: 9.7532
alpha: 90
beta: 90
gamma: 90
cell_volume: 267.842
crystal_density: 5.551
atoms_sites: ["Fe", "Cr1", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_y: gOIGAGB/FgAAAAAAAGscAAAdEAA=
atoms_z: QEIPAKBbBAAAAAAAQEIPAFBJJQA=
atoms_occupancy: 0
atoms_u_iso: 4FoBAAAyAADAXQAAAH0AAAB9AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure phase transitions in FeCr2O4 and structure analysis of new post-
 spinel FeCr2O4 and Fe2Cr2O5 phases with meteoritical and petrological implications

qdat:
AAAAAAAAAAAAAAAAAAAAAEgAEAAAAACAAAAAAAgkAAAigIAAQhQAAEEAAIiAAEAAEThAQIAACMCDCArAAgEAZ1AViBFgYjAYEhTUmAApAE1aIk0FkN8Dgs8ABDtlABwkDOLlRbASrxjUQANqAUrcWcOGg6AiOKDFKgFIDw==


formula: Zn.97 Fe.04 Al1.99 O4
compound: Jemaa, Kaduna, Nigeria
formula_title: <missing>
a: 8.0912
b: 8.0912
c: 8.0912
alpha: 90
beta: 90
gamma: 90
cell_volume: 529.711
crystal_density: 4.598
atoms_sites: ["ZnT", "FeT", "AlM", "FeM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAAgfEAA=
atoms_y: IKEHACChBwCAhB4AgIQeAAgfEAA=
atoms_z: IKEHACChBwCAhB4AgIQeAAgfEAA=
atoms_occupancy: QDQ7AMDUAQDgujwAIE4AAAAJPQA=
atoms_u_iso: cE4AAHBOAACQQgAAkEIAAEBCAAA=
atoms_aniso_label: ["ZnT", "FeT", "AlM", "FeM", "O"]
atoms_aniso_u11: cE4AAHBOAACQQgAAkEIAAEBCAAA=
atoms_aniso_u22: cE4AAHBOAACQQgAAkEIAAEBCAAA=
atoms_aniso_u33: cE4AAHBOAACQQgAAkEIAAEBCAAA=
atoms_aniso_u12: AAAAAAAAAACw+v//sPr///D7//8=
atoms_aniso_u13: AAAAAAAAAACw+v//sPr///D7//8=
atoms_aniso_u23: AAAAAAAAAACw+v//sPr///D7//8=
pub_title:
 Optical absorption spectroscopy study of the causes for color variations in natural
 Fe-bearing gahnite: Insights from iron valency and site distribution data
 Note: Sample Ni8967d


formula: Zn.91 Fe.1 Al1.98 Mg.01 O4
compound: Jemaa, Kaduna, Nigeria
formula_title: <missing>
a: 8.0954
b: 8.0954
c: 8.0954
alpha: 90
beta: 90
gamma: 90
cell_volume: 530.536
crystal_density: 4.576
atoms_sites: ["ZnT", "FeT", "AlM", "FeM", "MgM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAICEHgAIHxAA
atoms_y: IKEHACChBwCAhB4AgIQeAICEHgAIHxAA
atoms_z: IKEHACChBwCAhB4AgIQeAICEHgAIHxAA
atoms_occupancy: wIo3AEB+BQDAbDwAIE4AACBOAAAACT0A
atoms_u_iso: wEQAAMBEAABQNwAAUDcAAFA3AABQNwAA
atoms_aniso_label: ["ZnT", "FeT", "AlM", "FeM", "MgM", "O"]
atoms_aniso_u11: wEQAAMBEAABQNwAAUDcAAFA3AABQNwAA
atoms_aniso_u22: wEQAAMBEAABQNwAAUDcAAFA3AABQNwAA
atoms_aniso_u33: wEQAAMBEAABQNwAAUDcAAFA3AABQNwAA
atoms_aniso_u12: AAAAAAAAAACI+v//iPr//4j6//9o/P//
atoms_aniso_u13: AAAAAAAAAACI+v//iPr//4j6//9o/P//
atoms_aniso_u23: AAAAAAAAAACI+v//iPr//4j6//9o/P//
pub_title:
 Optical absorption spectroscopy study of the causes for color variations in natural
 Fe-bearing gahnite: Insights from iron valency and site distribution data
 Note: Sample Ni8967e

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAABAAAAAAAABAAAAIAAAAAAIAAAQAAAAAQAAEAAAABAABAAAACAAIAAABAAIAAAEABAAABAAgAACABAAAIAIAABACAABABAAAACAACAEAAIAgABAEAAQBAAEAgAAAQ==


formula: Zn.91 Fe.1 Al1.98 Mg.01 O4
compound: Migiandone mine, Val d'Ossola, Italy
formula_title: <missing>
a: 8.0944
b: 8.0944
c: 8.0944
alpha: 90
beta: 90
gamma: 90
cell_volume: 530.340
crystal_density: 4.578
atoms_sites: ["ZnT", "FeT", "AlM", "FeM", "MgM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAICEHgAgIBAA
atoms_y: IKEHACChBwCAhB4AgIQeAICEHgAgIBAA
atoms_z: IKEHACChBwCAhB4AgIQeAICEHgAgIBAA
atoms_occupancy: wIo3AEB+BQDAbDwAIE4AACBOAAAACT0A
atoms_u_iso: EFQAABBUAAAYRwAAGEcAABhHAABQRgAA
atoms_aniso_label: ["ZnT", "FeT", "AlM", "FeM", "MgM", "O"]
atoms_aniso_u11: EFQAABBUAAAYRwAAGEcAABhHAABQRgAA
atoms_aniso_u22: EFQAABBUAAAYRwAAGEcAABhHAABQRgAA
atoms_aniso_u33: EFQAABBUAAAYRwAAGEcAABhHAABQRgAA
atoms_aniso_u12: AAAAAAAAAADY+v//2Pr//9j6//+Q/P//
atoms_aniso_u13: AAAAAAAAAADY+v//2Pr//9j6//+Q/P//
atoms_aniso_u23: AAAAAAAAAADY+v//2Pr//9j6//+Q/P//
pub_title:
 Optical absorption spectroscopy study of the causes for color variations in natural
 Fe-bearing gahnite: Insights from iron valency and site distribution data
 Note: Sample Sp2781_6a


formula: Zn.7 Fe.35 Al1.92 Mg.03 O4
compound: Migiandone mine, Val d'Ossola, Italy
formula_title: <missing>
a: 8.1103
b: 8.1103
c: 8.1103
alpha: 90
beta: 90
gamma: 90
cell_volume: 533.471
crystal_density: 4.528
atoms_sites: ["ZnT", "FeT", "FeT", "AlM", "Fe3+M", "MgM", "Fe2+M", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAEAjEAA=
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAEAjEAA=
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAEAjEAA=
atoms_occupancy: gLkqAEBCDwBADQMAAJg6ACBOAABg6gAAgDgBAAAJPQA=
atoms_u_iso: eF8AAHhfAAB4XwAAsE8AALBPAACwTwAAsE8AALBPAAA=
atoms_aniso_label: ["ZnT", "FeT", "FeT", "AlM", "Fe3+M", "MgM", "Fe2+M", "O"]
atoms_aniso_u11: eF8AAHhfAAB4XwAAsE8AALBPAACwTwAAsE8AALBPAAA=
atoms_aniso_u22: eF8AAHhfAAB4XwAAsE8AALBPAACwTwAAsE8AALBPAAA=
atoms_aniso_u33: eF8AAHhfAAB4XwAAsE8AALBPAACwTwAAsE8AALBPAAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAA2Pr//9j6///Y+v//2Pr//xj8//8=
atoms_aniso_u13: AAAAAAAAAAAAAAAA2Pr//9j6///Y+v//2Pr//xj8//8=
atoms_aniso_u23: AAAAAAAAAAAAAAAA2Pr//9j6///Y+v//2Pr//xj8//8=
pub_title:
 Optical absorption spectroscopy study of the causes for color variations in natural
 Fe-bearing gahnite: Insights from iron valency and site distribution data
 Note: Sample Sp2781_6c

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAQAAAQAAAAAgAAIAAAACAACAAAAEAAQAAACAAQAAAIACAAAEABAAAEACAAAQAQAAEAEAACACAAAAIAAIAQAAQBAAEAQAAgEAAQBAAABA==


formula: Fe2.15 Cr.3 Al.22 Si.08 Mg.26 O4
compound: Synthetic
formula_title: <missing>
a: 9.8
b: 9.6
c: 2.87
alpha: 90
beta: 90
gamma: 90
cell_volume: 270.010
crystal_density: 5.269
atoms_sites: ["Fe1", "Cr1", "Al1", "Si1", "Fe2", "Mg2", "O1", "O2", "O3"]
atoms_x: 0EwaANBMGgDQTBoA0EwaAEBCDwBAQg8AgIQeAEBCDwBAEhcA
atoms_y: EKEmABChJgAQoSYAEKEmAADzFgAA8xYAgIQeAID1IADgyBAA
atoms_z: AAk9AAAJPQAACT0AAAk9AICEHgCAhB4AgIQeAAAJPQAACT0A
atoms_occupancy: gLkqAMAnCQDAtgYAAHECAMDGLQCA3g8AAAk9AAAJPQAACT0A
atoms_u_iso: IE4AACBOAAAgTgAAIE4AAIC7AACAuwAAAPQBAIAaBgDAVwEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis of a quenchable high-pressure form of magnetite (h-Fe3O4) with
 composition Fe1(Fe2+0.75Mg0.26)Fe2(Fe3+0.70Cr0.15Al0.11Si0.04)2O4
 Note: Sample Crystal 1

qdat:
AAAAAAAAAAAAAAAIAAAAAJAAAAAAAAEAABEAAAAAAACCABAAiAAAAAEEAAAAAgCQQEACBAAAAgEC4kQQGCBAEkQaQBAiEQAQ1QhEIEAIAiViI0MRICEFARIAEUREAoEAAEiQEkAACIkAAAJIAgyEARgAqjADSARZAoAAKS==


formula: Fe2.15 Cr.3 Al.22 Si.08 Mg.26 O4
compound: Synthetic
formula_title: <missing>
a: 9.8
b: 9.6
c: 2.87
alpha: 90
beta: 90
gamma: 90
cell_volume: 270.010
crystal_density: 5.269
atoms_sites: ["Fe1", "Cr1", "Al1", "Si1", "Fe2", "Mg2", "O1", "O2", "O3"]
atoms_x: 8FYEAPBWBADwVgQA8FYEAMDGLQDAxi0AUHD5/0BCDwAAAAAA
atoms_y: IDcIACA3CAAgNwgAIDcIALBXBwCwVwcA8J0NAIAsAwAAAAAA
atoms_z: AAk9AAAJPQAACT0AAAk9AICEHgCAhB4AAAk9AAAJPQCAhB4A
atoms_occupancy: gLkqAMAnCQDAtgYAAHECAMDGLQCA3g8AAAk9AAAJPQAACT0A
atoms_u_iso: oAMCAKADAgCgAwIAoAMCAIC1AQCAtQEAwF0AAIA4AQCAOAEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis of a quenchable high-pressure form of magnetite (h-Fe3O4) with
 composition Fe1(Fe2+0.75Mg0.26)Fe2(Fe3+0.70Cr0.15Al0.11Si0.04)2O4
 Note: Sample Crystal 2

qdat:
AAAAAAAAAAAAAAAIAAAAAJAAAAAAAAEAABEAAAAAAACCABAAiAAAAAEEAAAAAgCQQEACBAAAAgEC4kQQGCBAEkQaQBAiEQAQ1QhEIEAIAiViI0MRICEFARIAEUREAoEAAEiQEkAACIkAAAJIAgyEARgAqjADSARZAoAAKS==


formula: (Al.38 Ni.32 Fe.3)
compound: Khatyrka CV3 carbonaceous chondrite, Koryak Mountains, Russia
formula_title: <missing>
a: 3.0214
b: 3.0214
c: 3.0214
alpha: 90
beta: 90
gamma: 90
cell_volume: 27.582
crystal_density: 5.513
atoms_sites: ["Al", "Ni", "Fe"]
atoms_x: AAAAAAAAAAAAAAAA
atoms_y: AAAAAAAAAAAAAAAA
atoms_z: AAAAAAAAAAAAAAAA
atoms_occupancy: gDEXAACIEwCATxIA
atoms_u_iso: 8IEBAPCBAQDwgQEA
atoms_aniso_label: ["Al", "Ni", "Fe"]
atoms_aniso_u11: 8IEBAPCBAQDwgQEA
atoms_aniso_u22: 8IEBAPCBAQDwgQEA
atoms_aniso_u33: 8IEBAPCBAQDwgQEA
atoms_aniso_u12: AAAAAAAAAAAAAAAA
atoms_aniso_u13: AAAAAAAAAAAAAAAA
atoms_aniso_u23: AAAAAAAAAAAAAAAA
pub_title:
 Steinhardtite, a new body-centered-cubic allotropic form of aluminum from the
 Khatyrka CV3 carbonaceous chondrite

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAABAAAAAAAAAAAAAgAAAAAAAAAAEAAAAAAAAAAgAAAAAAAACAAAAAAAACAAAAAAAAgAAAAAAAgAAAAAACAAA==


formula: Sn.661 Cu2.652 S4
compound: Synthetic
pub_title: Preparation, crystal structure and electrical properties of Cu4SnS6
formula_title: <missing>
a: 3.739
b: 3.739
c: 32.941
alpha: 90
beta: 90
gamma: 120
cell_volume: 398.821
crystal_density: 4.687
atoms_sites: ["Sn", "Cu1", "Cu2", "S1", "S2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_z: AAAAAPB7AgDAcw0AAK0RAOCZHAA=
atoms_occupancy: IFgoAMDlEwAACT0AAAk9AAAJPQA=
atoms_u_iso: oIwAAAD6AABg6gAAgLsAAOCrAAA=
atoms_aniso_label: ["Sn", "Cu1", "Cu2", "S1", "S2"]
atoms_aniso_u11: AH0AACDLAAAA+gAAwNoAAOCrAAA=
atoms_aniso_u22: AH0AACDLAAAA+gAAwNoAAOCrAAA=
atoms_aniso_u33: 4KsAAIA4AQDA2gAAoIwAAOCrAAA=
atoms_aniso_u12: gD4AAGBtAAAAfQAAYG0AAMBdAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
qdat:
AAAAAAAAAEAAAAAAAAAgAAAAAAAACAAAEgBAgAAIAQAAAIAAAAAAAAAAhAAQAABACgiAEEAAgAAAAAAAAAAAADEgIIAIAAAAAkBAAQAAAAAAAAAAkCACDKCIBAAAAAAAAEoRAQAAAAAAA1CQEAAAUEBAAAAAAAAAADUKBA==


formula: Ba2 Ca Si4 B2 O14
compound: Itsi Range, Yukon Territory, Canada
formula_title: <missing>
a: 10.9515
b: 10.9515
c: 10.3038
alpha: 90
beta: 90
gamma: 90
cell_volume: 1235.790
crystal_density: 3.616
atoms_sites: ["Ba", "Ca", "Si", "B", "O1", "O2", "O3", "O4"]
atoms_x: sIQMAAAAAAAwah8AgIQeAIDBGADQNSIAUFoeABALJgA=
atoms_y: sIQMAAAAAAAYQAwAgEMUAIDBGABQaQ8A4HESACDABgA=
atoms_z: aPY8AHDWDgBgbg4AAAAAABAPBABA+wUA4BQVAACUEQA=
atoms_occupancy: 0
atoms_u_iso: 8JsAAMCPAAAwYQAAwEQAADB1AABAnAAAAK8AAMDaAAA=
atoms_aniso_label: ["Ba", "Ca", "Si", "B", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: aJIAAFB4AABAUQAAYCIAANBrAACQfgAAAMgAACDkAAA=
atoms_aniso_u22: aJIAAFB4AABwSQAA0FIAANBrAADwoAAAUJEAAPC5AAA=
atoms_aniso_u33: AK8AABC9AACAiQAA8FUAAPCHAAAgsgAA0LYAAKDwAAA=
atoms_aniso_u12: 4Pz//0Dt///A+f//AAAAACAcAADgFQAAcDAAADBcAAA=
atoms_aniso_u13: mA0AAAAAAABABgAAoA8AAGAJAABwFwAAUOL//yDR//8=
atoms_aniso_u23: mA0AAAAAAACwBAAAAAAAAGAJAABAOAAAIOr//6APAAA=
pub_title:
 Itsiite, Ba2Ca(BSi2O7)2, a new mineral species from Yukon, Canada: description
 and crystal structure

qdat:
AAAAAAAAAAAAAEgAAAAQIAACIAAhAAUAgBAAkQQAGBBIAogIBBCCFAQRCNIpFokFIiCCkhMhpUMKmSh0idfOiHSRChLropjzTHEutPc9Jy0la8bWiKB3qQ6SCDnIRnA6OgiYTEAIzAokBUAACAIgMQBAAAAAABCQAAAAAA==


formula: Fe4 O5
compound: Synthetic
formula_title: Fe4O5
a: 2.8964
b: 9.8225
c: 12.5808
alpha: 90
beta: 90
gamma: 90
cell_volume: 357.922
crystal_density: 5.630
atoms_sites: ["Fe1", "Fe2", "Fe3", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_y: AAAAAJA3EACw+R4AQMQKAECbFQDgdAUA
atoms_z: AAAAAIAUBwBAQg8AQEIPAODMIADwMycA
atoms_occupancy: 0
atoms_u_iso: oAkBAAB3AQDA1AEAAIn+/+AuAABAJf//
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and recovery of bulk Fe4O5 from magnetite, Fe3O4. A member of a self-
 similar series of structures for the lower mantle and transition zone

qdat:
AAAAAAAAAAAAAAAACAAAAIBAAAAgAAAABIAAACCEAQCEARBAIoogAAYAQACCAAkCkiWACsgAcAQLORAWAUUpsK3FBYMMLGAoVCtCCIVJA8axSsaDd8sBCPQZFU8GAKQ3BRZTSgyLAQwEJIQAjlW0MhDmh4ECYEp4SCAkJB==


formula: Cu3.296 Mg.704 Cl2 O6 H6
compound: Santo Domingo mine, Arica Province, Chile
pub_title: Tondiite, Cu3Mg(OH)6Cl2, the Mg-analogue of herbertsmithite Note: Sample IIa
formula_title: <missing>
a: 6.8345
b: 6.8345
c: 14.0022
alpha: 90
beta: 90
gamma: 120
cell_volume: 566.422
crystal_density: 3.514
atoms_sites: ["Cu1", "Cu2", "Mg2", "Cl", "O", "H"]
atoms_x: gIQeAAAAAAAAAAAAAAAAAPCZDAAATQgA
atoms_y: AAAAAAAAAAAAAAAAAAAAABBm8/8As/f/
atoms_z: AAAAAICEHgCAhB4AQNwLAPDKAwBAAQUA
atoms_occupancy: AAk9AAAREgAA+CoAAAk9AAAJPQAACT0A
atoms_u_iso: YJ8AAICJAACAiQAAMNkAAFDDAABg5AEA
atoms_aniso_label: ["Cu1", "Cu2", "Mg2", "Cl", "O"]
atoms_aniso_u11: kJcAAGCfAABgnwAAoPAAAMCoAAA=
atoms_aniso_u22: oIwAAGCfAABgnwAAoPAAAMCoAAA=
atoms_aniso_u33: YLgAAMBdAADAXQAAcK0AACD9AAA=
atoms_aniso_u12: UEYAALBPAACwTwAAUHgAAIBXAAA=
atoms_aniso_u13: iA4AAAAAAAAAAAAAAAAAALAdAAA=
atoms_aniso_u23: EB0AAAAAAAAAAAAAAAAAAFDi//8=
qdat:
AAAAAAAAAAAAAAAAAAAQAAEQAAAAAACAAABAQAoAAIAABAIIAQAEAQIMACAAgIIQQMAIAEUQIAgAhEEAggGAQCAExCAgiYjAgCJCBAJgAIRNGAEWBAgRIgALABCSSCAJEIEgAiEIAFohFJYQCkIJACFIgKliCUiShCTiAF==


formula: (Na.53 Ca.47) (Al.53 Fe.47) Si2 O6
compound: Synthetic
formula_title: <missing>
a: 9.616
b: 8.804
c: 5.274
alpha: 90
beta: 106.67
gamma: 90
cell_volume: 427.728
crystal_density: 3.474
atoms_sites: ["Na", "Ca", "Al", "Fe", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAAAAAALCdEQCA4gYAIPwVAFB3FQA=
atoms_y: wFUSAMBVEgBAMzcAQDM3ADCiBQBA6AQAIIoPALDMAAA=
atoms_z: QEIPAEBCDwBAQg8AQEIPABAFDgAANAgA8LESABAOAAA=
atoms_occupancy: QFkgAMCvHABAWSAAwK8cAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: kF8BAJBfAQCQyQAAkMkAANCdAAAwCwEA0BoBABDWAAA=
atoms_aniso_label: ["Na", "Ca", "Al", "Fe", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: QPoBAED6AQCQyQAAkMkAAGC4AAAAfQAAgDgBACDLAAA=
atoms_aniso_u22: wNoAAMDaAABQ3AAAUNwAAICiAAAAdwEAAPoAAKAJAQA=
atoms_aniso_u33: wAwBAMAMAQCAuwAAgLsAAKCMAACgCQEAYOoAAECcAAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAALAEAAAAAAAAgMH//7DS//8=
atoms_aniso_u13: oA8AAKAPAADQOQAA0DkAAMBEAAAQ9f//sAQAACAcAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAADD4//+gkv//0NX//+CY//8=
pub_title:
 Thermal expansion in C2/c pyroxenes: a review and new high-temperature structural
 data for a pyroxene of composition (Na0.53Ca0.47)(Al0.53Fe0.47)Si2O6 (Jd53Hd47)
 Note: T = 300 C

qdat:
AAAAAAAAAAAAAAAAEAAAAACBAAAABAAEBAAAQEAAAEQAIEIHAIAJCAAAARwgkBAQAhE4UBEoJCJZAAIEsANQmgK6CY4gkBn0IJD5JOijFM8KoJyANTpy0gqqp0pdoT7JDBvbb5TQkRtklskccsa45WKLisajPBnZd2UMET==


formula: (Na.53 Ca.47) (Al.53 Fe.47) Si2 O6
compound: Synthetic
formula_title: <missing>
a: 9.653
b: 8.858
c: 5.288
alpha: 90
beta: 106.76
gamma: 90
cell_volume: 432.950
crystal_density: 3.432
atoms_sites: ["Na", "Ca", "Al", "Fe", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAAAAAADCbEQDg6wYAAPkVAGBsFQA=
atoms_y: MFQSADBUEgAwJTcAMCU3AGCaBQCQ4wQAMH8PAJCwAAA=
atoms_z: QEIPAEBCDwBAQg8AQEIPAMDwDQDQOwgAkI8SABAOAAA=
atoms_occupancy: QFkgAMCvHABAWSAAwK8cAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0C0CANAtAgDwNgEA8DYBAPDrAACghgEAgLUBAOBBAQA=
atoms_aniso_label: ["Na", "Ca", "Al", "Fe", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: cNMCAHDTAgBQJwEAUCcBABAIAQDA2gAAAPQBAIA4AQA=
atoms_aniso_u22: EJ4BABCeAQCgVAEAoFQBAFD1AACgAwIAYGcBAKCGAQA=
atoms_aniso_u33: MKEBADChAQCgIgEAoCIBAEDOAACghgEA4KUBAHD4AAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAHAXAADA4P//4LH//2A7AAA=
atoms_aniso_u13: kOj//5Do//+QTAAAkEwAALBPAABAHwAAIE4AAEA4AAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAEAGAADgsf//0Lz//yCf//8=
pub_title:
 Thermal expansion in C2/c pyroxenes: a review and new high-temperature structural
 data for a pyroxene of composition (Na0.53Ca0.47)(Al0.53Fe0.47)Si2O6 (Jd53Hd47)
 Note: T = 700 C

qdat:
AAAAAAAAAAAAAAAAIAAAAACCAAAABAAICAAAgQAAAIQAQIQOAQASEAAAAhiBQBBACELIwCSgkFnSAAghwBTESAlEKXiBICvIhIVIZmSIJSghwsoC0+ubkFZLseF0Sq/EIJ7pnmVIaVIU3YNx6jytgzIkbFSbwreF/XBBCd==


formula: Pb O H I
compound: Synthetic
formula_title: Pb(OH)I
a: 7.8244
b: 4.2107
c: 10.4724
alpha: 90
beta: 90
gamma: 90
cell_volume: 345.026
crystal_density: 6.759
atoms_sites: ["Pb", "O", "H", "I"]
atoms_x: IAMyAKDFNQAAYy4AcGQhAA==
atoms_y: QEIPAMC98P/AvfD/QEIPAA==
atoms_z: sHwjAKDeHABABhkAYJETAA==
atoms_occupancy: 0
atoms_u_iso: oAkBAIA4AQBADQMAoAkBAA==
atoms_aniso_label: ["Pb", "O", "I"]
atoms_aniso_u11: 4KsAAMDUAQAgSAEA
atoms_aniso_u22: cPgAAMBdAAAg5AAA
atoms_aniso_u33: cHUBAIA4AQBA5wAA
atoms_aniso_u12: AAAAAAAAAAAAAAAA
atoms_aniso_u13: kGUAAMBj//9AHwAA
atoms_aniso_u23: AAAAAAAAAAAAAAAA
pub_title:
 Crystal structure of a novel synthetic compound, Pb2O(OH)I, and structure
 refinement of iodolaurionite, Pb(OH)I: hydroxo- and oxocentred units in Pb
 minerals and synthetic compounds

qdat:
AAAAAAAAAAAAAAAACAAAgAAAgABAEAgABICAEBAgwaQABAAIYiQJEGURmcAjgNABySZiCRSJw5YtMIo5q1GM/KJy3PhlNbfxPVM87Xa/PiVfp7eb2qvE3u+X/FrfWuaz/N/p/L3Lv2bvi/ne732N9bd8rdnh9svzRZb3uJ==


formula: Pb2 O2 H I
compound: Synthetic
formula_title: Pb2O(OH)I
a: 13.711
b: 4.0975
c: 9.584
alpha: 90
beta: 110.64
gamma: 90
cell_volume: 503.877
crystal_density: 7.571
atoms_sites: ["Pb1", "Pb2", "O1", "O2", "H1", "I"]
atoms_x: WDUJAFj9CQAgJg8AsJEOALCjCwCAiv//
atoms_y: gIQeAICEHgCAhB4AgIQeAICEHgCAhB4A
atoms_z: UPMgADimCACArhcAgIkyAEDuNQAQNw4A
atoms_occupancy: 0
atoms_u_iso: UEABAJB4AQBAlgEAQJYBAGBhAgBgmQEA
atoms_aniso_label: ["Pb1", "Pb2", "O1", "O2", "I"]
atoms_aniso_u11: YNEAADCIAQBAGQEAAPQBAIBRAQA=
atoms_aniso_u22: kEYBAMA+AQBgZwEA4KUBACAvAQA=
atoms_aniso_u33: 4KUBAAB3AQAgQgIAoIYBACApAgA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u13: 0GsAANBSAACgjAAAoAkBABByAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
pub_title:
 Crystal structure of a novel synthetic compound, Pb2O(OH)I, and structure
 refinement of iodolaurionite, Pb(OH)I: hydroxo- and oxocentred units in Pb
 minerals and synthetic compounds

qdat:
AAAAAAAAAAACAAAAIAAAAAAYAABAAAIADAAoAIIBAAAEAALAQgAQFCSGYAIEDQiBAZhcA0xAAEFKOrKBEqEoQB7QLMATWHAKeIfEohVUJzUKkSC7aJVDLTCzXOmuhAiFxjztGnZYgzsgx66SYQSoK3VVjJUwTNyYYkbQsR==


formula: Cu2 P O5 H
compound: Synthetic
pub_title: Low-temperature structural phase transition in synthetic libethenite Cu2PO4OH Note: T = 180 K
formula_title: <missing>
a: 8.0553
b: 8.3750
c: 5.8818
alpha: 90
beta: 90
gamma: 90
cell_volume: 396.805
crystal_density: 4.002
atoms_sites: ["Cu1", "Cu2", "P1", "O1", "O2", "O3", "O4", "H1"]
atoms_x: AAAAAKDp6f8IxfH/YNX3//Ak6/+wxPn/EHD4/0BD+v8=
atoms_y: gIQeAHDiFgC4Ww8AYCIZAGCWDgCAFAcAEEYYAEAqEwA=
atoms_z: CDQPAICEHgAAAAAAAAAAAADkDAAAAAAAgIQeAICEHgA=
atoms_occupancy: 0
atoms_u_iso: 0FIAALBoAAAgNQAAwEQAAPCHAACwzAAAkEwAAKAPAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAgAABgAAogARAAAAJACgAADQkBEiLIAAiiCgMbgIjEQKIBpdpeLECyRSeI31SylEtwt0iOh9txryuILi90KpPctzP7p/v+hz6/l5e/unsXU/v3/v139fr3v2/r9/dmnv/b9XyfWr/vrZ+r/7//q87==


formula: Cu2 P O5 H
compound: Synthetic
pub_title: Low-temperature structural phase transition in synthetic libethenite Cu2PO4OH Note: T = 120 K
formula_title: <missing>
a: 8.0545
b: 8.3622
c: 5.8755
alpha: 90
beta: 90.0012
gamma: 90
cell_volume: 395.735
crystal_density: 4.013
atoms_sites: ["Cu1", "Cu2", "P1", "O1", "O2", "O3", "O4", "O5", "H1"]
atoms_x: 4A89AHjyJgCYzy4AYN40AKCcJwAQvjYAwH01AADSKAAg+DcA
atoms_y: CIQeAGjlFgCgVQ8AUBQZAHAIDwCQCQcAkDkYAEAWDgCgIBIA
atoms_z: YDYPALhQHwBQXwAAUBQAAKCoDACQwwEAsGMeACDU8v/geh0A
atoms_occupancy: 0
atoms_u_iso: EEAAAHBJAABwMAAAkDMAALBoAABAUQAAMCoAADBDAADgqwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAgAAAAgAABAAAogARACAAIgCQBgiokAESHIAAiSBhcbAMikwNEBk946JECZI9dYzTSqlG/Y9yyORbd4r+WLN2r8K1n6lrv92+3mhx//39q7vn0Lrf7/68379f/9///q8/+1Tbv2fv7fbfvvvdXn/93/tef==


formula: (Mn1.8 Fe.2) Mo3 O8
compound: Shobu area, Ise City, Mie Prefecture, Japan
pub_title: Iseite, Mn2Mo3O8, a new mineral from Ise, Mie Prefecture, Japan
formula_title: <missing>
a: 5.8052
b: 5.8052
c: 10.2277
alpha: 90
beta: 90
gamma: 120
cell_volume: 298.499
crystal_density: 5.851
atoms_sites: ["Mn1", "Fe2", "Mn3", "Fe4", "Mo1", "O1", "O2", "O3", "O4"]
atoms_x: VVgUAFVYFABVWBQAVVgUAPDtCAAAAAAAVVgUAGA8HQDg8gkA
atoms_y: q7AoAKuwKACrsCgAq7AoABAS9/8AAAAAq7AoAKDD4v8gDfb/
atoms_z: MEU6ADBFOgCwwR8AsMEfAEBCDwAAahgAwKoIAOCkFgAAECcA
atoms_occupancy: gO42AIAaBgCA7jYAgBoGAAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAFAAQAAAAAQAAAAAAgQAAAmBAAAkAAAABAACYgAFAAEEYBBgACCAQQASxABAABRFokFACBEFIhQFVgjCCIQIlWAQIeTWZQEIDpFBIgEIgUpXgKIsWmSAiLoQphAkDoHQIUmtEAJOKDMSYICXgiP==


formula: Ca6 Al6.423 Fe.388 Si.189 O17.809 (Cl1.191 H3.618)
compound: Upper Chegem Caldera, Northern Caucasus, Russia
formula_title: <missing>
a: 12.0285
b: 12.0285
c: 12.0285
alpha: 90
beta: 90
gamma: 90
cell_volume: 1740.341
crystal_density: 2.945
atoms_sites: ["Ca1", "Al1", "Fe1", "Al2", "Si2", "O1", "O2", "Cl1", "Wat1"]
atoms_x: GAwJAAhWEAAIVhAAIKEHACChBwConxIAAEULAGDjFgBg4xYA
atoms_y: AAAAAAhWEAAIVhAAgIQeAICEHgAQEA0AAEULAAAAAAAAAAAA
atoms_z: QEIPAAhWEAAIVhAAQEIPAEBCDwBQahgAAEULAEBCDwBAQg8A
atoms_occupancy: AAk9AGAdNwCg6wUAoDA5AGDYAwAACT0AAAk9ACA7GADgzSQA
atoms_u_iso: 2MwAAFB4AABQeAAAoHMAAKBzAAAwPQEAsOUAAKDRAQCg0QEA
atoms_aniso_label: ["Ca1", "Al1", "Fe1", "Al2", "Si2", "O1", "O2", "Cl1", "Wat1"]
atoms_aniso_u11: wNoAAFB4AABQeAAAAGQAAABkAADwBAEAsOUAAOD2AADg9gAA
atoms_aniso_u22: wPMAAFB4AABQeAAAcHsAAHB7AAAgegEAsOUAAAA/AgAAPwIA
atoms_aniso_u33: IJkAAFB4AABQeAAAcHsAAHB7AADwNgEAsOUAAAA/AgAAPwIA
atoms_aniso_u12: AAAAAGgBAABoAQAAAAAAAAAAAAAAav//4OP//wAAAAAAAAAA
atoms_aniso_u13: AAAAAGgBAABoAQAAAAAAAAAAAABQl///4OP//wAAAAAAAAAA
atoms_aniso_u23: uB8AAGgBAABoAQAAAAAAAAAAAACg1wAA4OP//wAAAAAAAAAA
pub_title:
 Mayenite supergroup, part II: Chlorkyuygenite from Upper Chegem, Northern Caucasus,
 Kabardino-Balkaria, Russia, a new microporous mineral with "zeolitic" H2O

qdat:
AAAAAAAAAAAAAAAAAAAAAIAACAAAAAAAEABAAAAgBACAIAACAIAAACAgIAAgIEBAgQAAECCBBBBABBABCCCAIIQghCAIAiCIQCEABEIBEQCIgEAEREBABEAAiIEQAgAAgAAAgAAAAAAABIAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Be2 Si O4
compound: natural crystal from unreported locality
formula_title: <missing>
a: 12.485
b: 12.485
c: 8.264
alpha: 90
beta: 90
gamma: 120
cell_volume: 1115.573
crystal_density: 2.950
atoms_sites: ["Be1", "Be2", "Si1", "O1", "O2", "O3", "O4"]
atoms_x: 0P07AIgOPAAQDjwAQGMHABgBAAAIwDcAeK83AA==
atoms_y: sNoLANjaCwBo8AsAGMwMAFBaFAAYdwcAsHUHAA==
atoms_z: AF8ZAEAkBQBgxy0AYMItAEDJLQD41DcAQLUjAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Be1", "Be2", "Si1", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: IEkAADBIAAAIJQAAQEcAAJhOAAAoPAAAcEQAAA==
atoms_aniso_u22: MEgAAAhXAADIKAAAiGgAAHg3AADwMgAACD4AAA==
atoms_aniso_u33: oEsAAJhEAACIIgAACC8AAHBOAAB4PAAAmDAAAA==
atoms_aniso_u12: IBcAAGAsAABgEwAAiDYAAPglAABYBwAA2A4AAA==
atoms_aniso_u13: CAcAAAAAAAA4////APv//yj2//9oAQAAaPz//w==
atoms_aniso_u23: aAEAAMD0///QAgAAaPz//wAAAACY/v//YPr//w==
pub_title:
 An X-ray diffraction study of the electron-density distribution and
 electrostatic potential in phenakite Be2SiO4

qdat:
AAAAAAAAAAAAAAAAhAAAAAAQAAAQEgABAEAAgQgABEAQoAIBAIqCBAKIBQUEMEARSAwQIkQkoQoAzTEBIcEzCKMwyKBwtUobVyWRzlkZVOFS25jGtStLLvF6MquWCgXq/cLNciVeS1AXS1F+XgAOumBtyopHZAGFIWwqgA==


formula: Pt7 Cu
compound: Lubero region, North Kivu, Congo
formula_title: <missing>
a: 7.7891
b: 7.7891
c: 7.7891
alpha: 90
beta: 90
gamma: 90
cell_volume: 472.565
crystal_density: 20.087
atoms_sites: ["Pt1", "Pt2", "Cu"]
atoms_x: gIQeAAAAAAAAAAAA
atoms_y: gIQeAEBCDwAAAAAA
atoms_z: gIQeAEBCDwAAAAAA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kitagohaite, Pt7Cu, a new mineral from the Lubero region, North Kivu,
 Democratic Republic of the Congo

qdat:
AAAAAAAAAAAAAAAAAAAAAAAIAABAAAAAAAAAAAgAAAAACAEAAAAAABAAAACAQAAAABAAABAAAAAAgAAECAAAAgAAQQAAAQAAggAACAAIAAAEAAhAAAgAIQAAQAEQAAQAIAACACEAAQAiAAAARAAIAQAAgBEABAEQAIAgAB==


formula: Pb As Cu (O5 H)
compound: Cassiterite-sulfide field, Festivalnyi, East Siberia, Russia
pub_title: Study of crystalline structures of rare arsenates: duftite and mimetite
formula_title: <missing>
a: 7.770
b: 9.209
c: 5.995
alpha: 90
beta: 90
gamma: 90
cell_volume: 428.966
crystal_density: 6.607
atoms_sites: ["Pb", "As", "Cu", "O-H1", "O2", "O3", "O4", "O5"]
atoms_x: IKEHAEDvBwDAgA8A4AQHACDhJgBA2zQAIKYbACCmGwA=
atoms_y: YDEKAEA+MQBAZR4AQH0aACCfMQCAbQ0AYJUjAMCKNwA=
atoms_z: AAAAAGDkAQDAAw8AQJwAAEBIDgBgDRAAgNA7AMDOAgA=
atoms_occupancy: 0
atoms_u_iso: gKsBAHgtAABIngAAYDsAAIDtAAAgsgAAILIAAGhQAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAACABAAgCQACAAgoAEAYCCAFQEBACGGABFCbAZmgggA5wYQQQJ2SicPJjFvQLXOdkByz/1Q4zC/hWmP6K99cD3Vf997vfevnT7/ql361b3b697PVf85/+3N2/9//0/99f/t1++f+3vVL//3/8x==


formula: Pb5 As3 O12 Cl
compound: Cassiterite-sulfide field, Festivalnyi, East Siberia, Russia
pub_title: Study of crystalline structures of rare arsentates: duftite and mimetite
formula_title: <missing>
a: 10.248
b: 10.248
c: 7.441
alpha: 90
beta: 90
gamma: 120
cell_volume: 676.769
crystal_density: 7.303
atoms_sites: ["Pb1", "Pb2", "As", "O1", "O2", "O3", "Cl"]
atoms_x: EMw8AFVYFACg9hgAwJ4KAMB/JACgixUAAAAAAA==
atoms_y: YL0tAKuwKACghgEAIBceAGDGBgDgjQUAAAAAAA==
atoms_z: QEIPABByAABAQg8AQEIPAEBCDwDARQQAgOkiAA==
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQAACT0AgIQeAA==
atoms_u_iso: UP8AANDPAAA4TwAAwFECAGAWAgAI8AIA8FIDAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAABAAAAAAIAEAACBAAEQAEQAARICAQABAkRBQBQIKAkEIgxIEDhioFIoKEUGCFOUWYoQozAANe5nYNSSi0VzfumODFZvJz5Ppy525dTsdPkz+1ncJj377a+/yeNfmvbn5g3F63/ZvVqtb94ut5rzPnZ0TBc8V==


formula: Ba3 V2 O8
compound: Synthetic
formula_title: <missing>
a: 5.7811
b: 5.7811
c: 21.2886
alpha: 90
beta: 90
gamma: 120
cell_volume: 616.167
crystal_density: 5.189
atoms_sites: ["Ba1", "Ba2", "V1", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAACDlHQA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAOAjHwA=
atoms_z: AAAAAMCCMADwLCQAoMgoAMA7DgA=
atoms_occupancy: 0
atoms_u_iso: IAcBACAHAQA4TwAAcFIBAHBSAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry, Rietveld refinements and Raman spectroscopy studies of the
 new solid solution series: Ba3-xSrx(VO4)2 (0<=x<=3)
 Note: x = 0

qdat:
AAAAAAAAAAAAAABAAAAAAEAQAAAACEAAIAAAQAAQIAQgMASAEAAAAEQEQUCAEABAEQABAIAAEAgChAoIAABBRQgQAAkKEIIBAkAIIAAECiEECCRSGIAFFMQgAUBAAEMKDECFAxAAEVEIAICAAiGBEAJUhAGBAAiACAAKkQ==


formula: (Ba2.5 Sr.5) V2 O8
compound: Synthetic
formula_title: <missing>
a: 5.7617
b: 5.7617
c: 21.1048
alpha: 90
beta: 90
gamma: 120
cell_volume: 606.755
crystal_density: 5.066
atoms_sites: ["Ba1", "Sr1", "Sr2", "Ba2", "V1", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgO4dAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgBofAA==
atoms_z: AAAAAAAAAABwhzAAcIcwABAwJADQ2SgAcEAOAA==
atoms_occupancy: QOcyAMAhCgBgMQoAoNcyAAAJPQAACT0AAAk9AA==
atoms_u_iso: KAkBACgJAQAoCQEAKAkBADhPAACQRgEAkEYBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry, Rietveld refinements and Raman spectroscopy studies of the
 new solid solution series: Ba3-xSrx(VO4)2 (0<=x<=3)
 Note: x = 0.5

qdat:
AAAAAAAAAAAAAABAAAAAAEAQAAAABBAAEAAAIAAICAIQDAEgBAAAABEBIDAgBAAgCkAAQCAACAUBIQMCAAAIUIIEAAFChCBAQNACCAAAQohBAgUURhAAopEEADAEABBigYghICIAAhohAAgQAEYoMgBGyIAwEAEQAQAA0R==


formula: (Ba2 Sr) V2 O8
compound: Synthetic
formula_title: <missing>
a: 5.7362
b: 5.7362
c: 20.9041
alpha: 90
beta: 90
gamma: 120
cell_volume: 595.677
crystal_density: 4.952
atoms_sites: ["Ba1", "Sr1", "Sr2", "Ba2", "V1", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA0OkdAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAMB8fAA==
atoms_z: AAAAAAAAAABAjzAAQI8wAHA5JABg2ygAYDIOAA==
atoms_occupancy: 4CwqACDcEgBwFhUAkPInAAAJPQAACT0AAAk9AA==
atoms_u_iso: MAEBADABAQAwAQEAMAEBABBZAABIXAEASFwBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry, Rietveld refinements and Raman spectroscopy studies of the
 new solid solution series: Ba3-xSrx(VO4)2 (0<=x<=3)
 Note: x = 1

qdat:
AAAAAAAAAAAAAAAgAAAAACAIAAAAAQgACAAAEAAEAgEIAYCIAgAAAAJAiAwIAQAQAlAACAgAAgEgSCEggAACFBiAgAAokIgQCBoAIQAACFEIIEEihKIAClEggAMAgAEKKBiCEgYgACMSEAEBAARjAyACpIgBgQARgAgACp==


formula: (Ba1.5 Sr1.5) V2 O8
compound: Synthetic
formula_title: <missing>
a: 5.7084
b: 5.7084
c: 20.6912
alpha: 90
beta: 90
gamma: 120
cell_volume: 583.909
crystal_density: 4.840
atoms_sites: ["Ba1", "Sr1", "Sr2", "Ba2", "V1", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA0AIeAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAMAYfAA==
atoms_z: AAAAAAAAAADwkzAA8JMwAOA3JABg2ygA0DAOAA==
atoms_occupancy: 4FwiACCsGgCwcCAAUJgcAAAJPQAACT0AAAk9AA==
atoms_u_iso: MAsBADALAQAwCwEAMAsBAAhhAACQpQEAkKUBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry, Rietveld refinements and Raman spectroscopy studies of the
 new solid solution series: Ba3-xSrx(VO4)2 (0<=x<=3)
 Note: x = 1.5

qdat:
AAAAAAAAAAAAAAAQAAAAABAEAAAAAIIAAgAACAACAICEAGAiAIAAAABQIgGCAEAEAIoAAQEAAIAkEgQkEAAARIMQIAADFBEBAgTABCAAAIoRAgQSUIxAAMoSCAAwCAAgowKIISAiAAIooQAICACFMDIAFShADAgBCgBAAF==


formula: (Ba Sr2) V2 O8
compound: Synthetic
formula_title: BaSr2(VO4)2
a: 5.6792
b: 5.6792
c: 20.4821
alpha: 90
beta: 90
gamma: 120
cell_volume: 572.110
crystal_density: 4.723
atoms_sites: ["Ba1", "Sr1", "Sr2", "Ba2", "V1", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIBceAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA4PEeAA==
atoms_z: AAAAAAAAAAAwmjAAMJowAEBBJABQ5igA0DAOAA==
atoms_occupancy: YGAXAKCoJQCwNCoAUNQSAAAJPQAACT0AAAk9AA==
atoms_u_iso: iEQBAIhEAQCIRAEAiEQBAIiQAADg3AEA4NwBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry, Rietveld refinements and Raman spectroscopy studies of the
 new solid solution series: Ba3-xSrx(VO4)2 (0<=x<=3)
 Note: x = 2

qdat:
AAAAAAAAAAAAAAAIAAAAABACAAAAAECAAIAABAAAgCBBAAwQgCAAAAAKEIAggBABACGAACBAABAIQkCFAgAACJBkAgAAIoEgICBMAEIAAAkhIECCJQlEAAShIIADAIACCSgYghIBEAAShQgAQEAEKYKQALEiAGBABFACAA==


formula: (Ba.5 Sr2.5) V2 O8
compound: Synthetic
formula_title: Ba.5Sr2.5(VO4)2
a: 5.6498
b: 5.6498
c: 20.2789
alpha: 90
beta: 90
gamma: 120
cell_volume: 560.585
crystal_density: 4.600
atoms_sites: ["Ba1", "Sr1", "Sr2", "Ba2", "V1", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA8B4eAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEOoeAA==
atoms_z: AAAAAAAAAAAgpTAAIKUwALA/JABACikAEDcOAA==
atoms_occupancy: gHkLAICPMQCAgzMAgIUJAAAJPQAACT0AAAk9AA==
atoms_u_iso: QPsAAED7AABA+wAAQPsAAChLAAAAcgEAAHIBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry, Rietveld refinements and Raman spectroscopy studies of the
 new solid solution series: Ba3-xSrx(VO4)2 (0<=x<=3)
 Note: x = 2.5

qdat:
AAAAAAAAAAAAAAAEAAAAAAgBAAAAABAgAEAAAgAAQAgQgAEEIAgAAAABhEAEIAQAQAgwAAQIAAQCCJARIIAAASIEQIAABFAkBAgIgAhAAACUEgQQIqCUQABKEggAEAQAIJKBSCEQCQAAVFCAAgIAITQUgAWOEAEBACJAEA==


formula: Sr3 V2 O8
compound: Synthetic
formula_title: Sr3(VO4)2
a: 5.6214
b: 5.6214
c: 20.0997
alpha: 90
beta: 90
gamma: 120
cell_volume: 550.059
crystal_density: 4.462
atoms_sites: ["Sr1", "Sr2", "V1", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAFAoHgA=
atoms_y: AAAAAAAAAAAAAAAAAAAAALDgHgA=
atoms_z: AAAAAPCsMAAQSSQAUDEpAFA9DgA=
atoms_occupancy: 0
atoms_u_iso: EA0BABANAQD4BwAAqJcBAKiXAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry, Rietveld refinements and Raman spectroscopy studies of the
 new solid solution series: Ba3-xSrx(VO4)2 (0<=x<=3)
 Note: x = 3

qdat:
AAAAAAAAAAAAAAACAAAAAAQBAAAAAAgIABAAAIAAIAIIIABBCAIAAAAAIRABCACAEAIEAAECAAEAQSIBJBAAACSAkBAAAFICgIEBCACIAAAKgUCBBEoKhAAFQUCAAQBAAgiwFEIJAJAABYMEACAQARLAxAA0UIAICAISAI==


formula: Na Pb2 C2 (O7 H)
compound: Synthetic
pub_title: Synthesis and crystal structure of new carbonate NaPb2(CO3)2(OH)
formula_title: <missing>
a: 5.268
b: 5.268
c: 13.48
alpha: 90
beta: 90
gamma: 120
cell_volume: 323.975
crystal_density: 5.888
atoms_sites: ["Na1", "Pb1", "Pb2", "C1", "C2", "O-H1", "O2", "O3"]
atoms_x: q7AoAKuwKACrsCgAAAAAAAAAAACrsCgAYDcJAIDYEAA=
atoms_y: VVgUAFVYFABVWBQAAAAAAAAAAABVWBQAAJQRACCbCAA=
atoms_z: cHw2ACD/IQAgyA0A4CICAIDYEACArhcAALcgAOAULgA=
atoms_occupancy: 0
atoms_u_iso: sDoBAEioAAAgsgAACFcAAEg/AADwIgEAgO0AADikAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAEAAAAAAAgQAACAAAgCAAAAACCAACAARGAEAEEgAAEAAAgSYSAAkQARIEQiFAEEKAkAkCSQIhRIAQJVQCgAgSipQClBUKKICJQQFBlARFIQW0TAIKliBlEAiMAkBEnUUoaQ2CQkDFoJKEEQEgljEpiAN==


formula: Rh As
compound: Synthetic
pub_title: Arsenides of the transition metals IV. A note on the platinum metal arsenides
formula_title: <missing>
a: 5.62
b: 3.58
c: 6.00
alpha: 90
beta: 90
gamma: 90
cell_volume: 120.718
crystal_density: 9.784
atoms_sites: ["Rh", "As"]
atoms_x: QA0DAEDRDAA=
atoms_y: QEIPAEBCDwA=
atoms_z: QNEMAIBmIwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAhAAIBEAQAAAAAIAQEgAAAEAAFAgABBIEgAQJCEYAEAECgQiAqAIABIQMAoghjqIgEcAkQDCEbCJBJdASBUNyWCqFpFgaVqFUJlKEbhSFaFdLQTtBcbMQfF1aErtk8TbtBQ0f==


formula: Fe2.668 O4
compound: Synthetic
formula_title: <missing>
a: 8.3474
b: 8.3474
c: 8.3474
alpha: 90
beta: 90
gamma: 90
cell_volume: 581.639
crystal_density: 4.864
atoms_sites: ["Fe1", "Fe2", "Fe3", "O1", "O2"]
atoms_x: kI08AKDLNABg4xYAII00AIC0FgA=
atoms_y: kI08AGCJJQAgoQcAII00AKACFwA=
atoms_z: kI08AOBnNQDgZzUAII00AIB3NQA=
atoms_occupancy: AAk9AAAJPQBgchQAAAk9AAAJPQA=
atoms_u_iso: EFkAABBZAAAQWQAAEFkAABBZAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Vacancy ordering in gamma-Fe2O3: synchrotron x-ray powder diffraction and high-
 resolution electron microscopy studies

qdat:
AAAAAAAAAAAAAAAAAAAAACAAAAAAgACAAAAAACAAACAAAQAgAAQCAACAAEBAAACAAQAECAAggAQAIIAIIAIAQQBBCEAIQBCAIAhAIRCAQgEQiARARAICICIiAiBERASAkRAkAIkCIIkQRAkCCQJJAkEkgSCSQCAQQSCEgk==


formula: Fe2.645 O3.99
compound: Synthetic
formula_title: <missing>
a: 8.3364
b: 8.3364
c: 8.3364
alpha: 90
beta: 90
gamma: 90
cell_volume: 579.343
crystal_density: 4.851
atoms_sites: ["Fe1", "Fe2", "Fe3", "O1", "O2"]
atoms_x: QLv//6AlJgAgoQcAEEwXABBMFwA=
atoms_y: QLv//6AlJgDQZBYAEEwXAABSNQA=
atoms_z: QLv//6AlJgBw5jUAEEwXALDTNQA=
atoms_occupancy: AAk9AMBcFQCA0DsAwGw8AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Neutron and X-ray diffraction study of ferrite nanocrystals obtained by
 microwave-assisted growth. A structural comparison with the
 thermal synthetic route

qdat:
AAAAAAAAAAAAAAAAAAAAABAAAAAAQABAAAAEACAAACAAAIAgAAIBAABAQEAgAEBAgIACBAAgQAIAEIAEIIIAQQAghCEEIAhAEARAEIhEIgEIhAQgIQEREBERARASIiRASIgRACRIkCRIEgiCAkEkgSBJIJBJIAgIJJBBIR==


formula: Fe2.645 O3.99
compound: Synthetic
pub_title: A study on the structure of maghemite (gamma-Fe2O3) I. Rietveld analysis of powder XRD patterns
formula_title: <missing>
a: 8.3457
b: 8.3457
c: 8.3457
alpha: 90
beta: 90
gamma: 90
cell_volume: 581.284
crystal_density: 4.835
atoms_sites: ["Fe1", "Fe2", "Fe3", "O1", "O2"]
atoms_x: oCUmAEC7//8goQcAEEwXABBMFwA=
atoms_y: oCUmAEC7///QZBYAEEwXAABSNQA=
atoms_z: oCUmAEC7//9w3fj/EEwXALDTNQA=
atoms_occupancy: wFwVAAAJPQCA0DsAwGw8AAAJPQA=
atoms_u_iso: 6GIAAHiMAAB4jAAAmIoAAEieAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAACAAAAAAgACAAAAEACAAACAAAQAgAAQCAACAQEBAAECAgQAECAAggAQAIIAIIIIAQQBBCEEIQBCAIAhAIQiEQgEQiARAQgIiICIiAiBERERAkRAkAIkSIEkQRAkCCIJJAkEkgSCSQCAQSSCEgU==


formula: As2 Te3
compound: Synthetic
pub_title: The crystal structure and powder data for arsenic telluride
formula_title: <missing>
a: 14.339
b: 4.006
c: 9.873
alpha: 90
beta: 95.0
gamma: 90
cell_volume: 564.967
crystal_density: 6.262
atoms_sites: ["As1", "As2", "Te1", "Te2", "Te3"]
atoms_x: 4AQHACCDDAAA9AEAABcRAGDjFgA=
atoms_y: gIQeAAAAAAAAAAAAgIQeAAAAAAA=
atoms_z: ICkbAKDZCABANhEAoJEUAEATAgA=
atoms_occupancy: 0
atoms_u_iso: sO4BALDuAQCw7gEAsO4BALDuAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAACAAACAAABAAIAAAABQAIAAgARAICAAAQMAgwQggAEwIZIEUiDIsIAjVABEoTggyIWmAwVEyNOCDSCCwtkpVepFQjZY0JuPHjWlj8mbRaoVecXTDAmDcqg7LCksmwNFvRIHZVCVY0sphQhnAhgAf26UgonOCD==


formula: As2 Te3
compound: Synthetic
pub_title: Crystal structure of arsenic telluride As2Te3
formula_title: <missing>
a: 14.364
b: 4.025
c: 9.889
alpha: 90
beta: 95.14
gamma: 90
cell_volume: 569.435
crystal_density: 6.213
atoms_sites: ["As1", "As2", "Te1", "Te2", "Te3"]
atoms_x: uNcGANBpDACoyQEAQP8QAPjSFgA=
atoms_y: gIQeAAAAAAAAAAAAgIQeAAAAAAA=
atoms_z: aPUaAKifCACQhhEAOL0UAJAnAgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["As1", "As2", "Te1", "Te2", "Te3"]
atoms_aniso_u11: 2NUBAKh0AQCQIwEAKFQBAODiAAA=
atoms_aniso_u22: aM4AAKCqAAB4eAAAIEkAAMBiAAA=
atoms_aniso_u33: 6H8BAEhhAQBgjwEAEBwBAIBCAQA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u13: sL0AALAsAACwLAAAWBYAABgLAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
qdat:
AAAAAAAAAACAAACAAABAAIAAAABgAIABgAhAICAAAQMBBQRAgAEggSgI8kEKUwBppACRQ3BAkQ5qBQoRiqsCLiUVBfJSstMSiGxywNUqel5GXyaqllA2zxOoPCwORjFS0NpTXA4Zy5AVKoinY5aMRCPSEEAD3dlIMF1YxQ==


formula: As2 Te3
compound: Synthetic
pub_title: Hydrothermal growth and the crystal structure of arsenic telluride, As2Te3
formula_title: <missing>
a: 14.3573
b: 4.0199
c: 9.8990
alpha: 90
beta: 95.107
gamma: 90
cell_volume: 569.052
crystal_density: 6.217
atoms_sites: ["As1", "As2", "Te1", "Te2", "Te3"]
atoms_x: oF0MAFDqBgCQwwEAEPMQAADaFgA=
atoms_y: AAAAAICEHgAAAAAAgIQeAAAAAAA=
atoms_z: AJgIAGDkGgBAgREA4LAUALAqAgA=
atoms_occupancy: 0
atoms_u_iso: aPEAAOAeAQDQzwAAAL4AAOjBAAA=
atoms_aniso_label: ["As1", "As2", "Te1", "Te2", "Te3"]
atoms_aniso_u11: oFQBALBJAQAg5AAAMPIAAAD6AAA=
atoms_aniso_u22: UMMAAGAcAQCQsAAAAJYAAACvAAA=
atoms_aniso_u33: 8LkAAHD4AADA2gAA0LYAANCdAAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u13: MEMAAKBBAADAKwAA0O7//zD4//8=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
qdat:
AAAAAAAAAACAAACAAABAAQAAAABgAIABgAhAYCAAAQMAgwRAgAFgQSQI8kCJUwBHqACJQzBBkQ5iBgsJmecEMiKNBfJIs9SUhOiywVYqdT5GPyZrG9hr0pMsOCYOSlFqoPUyfAUJ7NAalYJXks2GJCPMEGACyvikLG64QQ==


formula: As2 Te3
compound: Synthetic
pub_title: Polymorphism in thermoelectric As2Te3 Note: T = 300 K
formula_title: <missing>
a: 14.337
b: 4.015
c: 9.887
alpha: 90
beta: 95.06
gamma: 90
cell_volume: 566.908
crystal_density: 6.241
atoms_sites: ["As1", "As2", "Te1", "Te2", "Te3"]
atoms_x: EOQGAKBEDACQwwEAwPcQALDeFgA=
atoms_y: gIQeAAAAAAAAAAAAgIQeAAAAAAA=
atoms_z: QOEaAACYCABAmhEA4MkUADA3AgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAACAAACAAABAAIAAAABQAIABgARAICAAAQMAgwQggAEwQSQEsiCJMQAlZACIwyggmI8mBwUJSdeCGSKEhLlKaUqSgmRxoKsdPK8mL5MmjWw16YmmHBMHZTBmWFqZXgaI+SgMzMEzxmSjEhDWCDABdWqRDjVcMU==


formula: As2 Se3
compound: Synthetic
pub_title: A new polymorphic modification of arsenic selenide obtained at high presssures
formula_title: As2Se3
a: 13.37
b: 3.73
c: 9.31
alpha: 90
beta: 95
gamma: 90
cell_volume: 462.524
crystal_density: 5.554
atoms_sites: ["As1", "As2", "Se1", "Se2", "Se3"]
atoms_x: IIMMAOAEBwAA9AEAABcRAGDjFgA=
atoms_y: AAAAAICEHgAAAAAAgIQeAAAAAAA=
atoms_z: oNkIACApGwBANhEAoJEUAEATAgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAIAAACAAAAQAEAAAAACQAEABIACIEgIAAAQQAQYUIIAApAUYIDMhBiZFApWgBAiIrATRjqaRUCNJhN+gNKBgk8eg4IjDiA3coCTklVZckPyuKNCxTgzD0cOSDbrBkCxY4gSaPwZxeJhQpFAThDMUmSIyyBQQ==


formula: Fe2.667 O4
compound: Synthetic
formula_title: <missing>
a: 8.4053
b: 8.4053
c: 8.4053
alpha: 90
beta: 90
gamma: 90
cell_volume: 593.827
crystal_density: 4.764
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: IKEHAICEHgAAVQ8A
atoms_y: IKEHAICEHgAAVQ8A
atoms_z: IKEHAICEHgAAVQ8A
atoms_occupancy: oMs0ACD+NgAACT0A
atoms_u_iso: AOEAAADhAAAwiAEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Formation of gamma-Fe2O3 nanoparticles and vacancy ordering: an in situ
 X-ray powder diffraction study

qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAIAAAAAIAAAAAAABAAAAIAAAAAAgAACAAAAAEAACAAAABAACAAAAIAAgAAAQACAAACAAgAACABAAAEAEAABABAAAgAgAAgBAAAACAAEAQAAgEAAIBAAEAgACAgAAAQAEBAAA==


formula: Fe3 O4
compound: Natural, not provided
pub_title: The structure of magnetite: Symmetry of cubic spinels Note: Sample 633A
formula_title: <missing>
a: 8.3941
b: 8.3941
c: 8.3941
alpha: 90
beta: 90
gamma: 90
cell_volume: 591.456
crystal_density: 5.200
atoms_sites: ["Fe1", "Fe2", "Fe3", "O1", "O2"]
atoms_x: AAAAAICEHgBQKiYAIDw1ABBMFwA=
atoms_y: AAAAAICEHgBQKiYAIDw1ABBMFwA=
atoms_z: AAAAAICEHgBQKiYAIDw1ABBMFwA=
atoms_occupancy: 0
atoms_u_iso: iEUAAKhDAACYXQAAUEYAAFidAAA=
atoms_aniso_label: ["Fe1", "Fe2", "Fe3", "O1", "O2"]
atoms_aniso_u11: sEUAAIBDAADAXQAAUEYAAFidAAA=
atoms_aniso_u22: sEUAAIBDAADAXQAAUEYAAFidAAA=
atoms_aniso_u33: sEUAAIBDAADAXQAAUEYAAFidAAA=
atoms_aniso_u12: AAAAAAAAAAAACgAAiBgAAPDJ//8=
atoms_aniso_u13: AAAAAAAAAAAACgAAiBgAAPDJ//8=
atoms_aniso_u23: AAAAAAAAAAAACgAAiBgAAPDJ//8=
qdat:
AAAAAAAAAAAAAAAAAAAAACAAAgAAAAAAAAAIAAAAAIAQAAAAABAAAAIBAAAAAQAABAAAAAEAABBAAABAABCAAAEAAggAAIABAAABAAhAABAAhAACACIAAgAgAAIASAAQAiAAACIACAIAAQBIAEASACAIABAIAAARACASAA==


formula: Be
compound: Synthetic
pub_title: Diffraction study of the electron density distribution in beryllium metal
formula_title: <missing>
a: 2.2853
b: 2.2853
c: 3.5842
alpha: 90
beta: 90
gamma: 120
cell_volume: 16.211
crystal_density: 1.846
atoms_sites: ["Be"]
atoms_x: VVgUAA==
atoms_y: q7AoAA==
atoms_z: QEIPAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAEAEAAAAAAAAAAAAAAAAABAAAAAAAAAAAACAAAAAAAAAAIAABAACBAAAAAABAAABAAAAAAAIAAAAAAAAIAAgAAgAAAAEAACAAAIACCAAAAAAQ==


formula: B
compound: Synthetic
pub_title: Electron deformation density in alpha-boron Note: alpha-phase
formula_title: <missing>
a: 4.9179
b: 4.9179
c: 12.5805
alpha: 90
beta: 90
gamma: 120
cell_volume: 263.504
crystal_density: 2.453
atoms_sites: ["B1", "B2"]
atoms_x: MEEHAPADDAA=
atoms_y: 0Mc1ABAFMQA=
atoms_z: CGc2AAB8AQA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAggAACAAAAAAAAAAAIEAAAAAIJgAgAAAAAAIAAAQECAQAAAgAhAgQRAAAABAAQRICgQAAQCACBDCAAABAShEEABASIIkAACAACgQQAQKBBYQAAQKiRABBAEQAAQElCEAQMESAAAAUEQCEE==


formula: B25
compound: Synthetic
formula_title: <missing>
a: 8.708
b: 8.708
c: 5.0750
alpha: 90
beta: 90
gamma: 90
cell_volume: 384.834
crystal_density: 2.332
atoms_sites: ["B1", "B2", "B3", "B4", "B5"]
atoms_x: AAAAAPCPBwCgAA8AEEsTAAD3DQA=
atoms_y: AAAAAPCPBwCgAA8AIFwGADAMBQA=
atoms_z: gIQeANB9FgAQ/iMAsNgXALD/BAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High pressure synthesis and investigation of single crystals
 of metastable boron phases
 Note: alpha-tetragonal phase

qdat:
AAAAAAAAAAAAAAAAAgAAAAABgAAAAAAAABgAAAgAAMAACAABwAAgAHAAQAAAAIAsACAFgAQCQBACgAAOAIEYQguAAMhCAAEFwgFQEChFHAC0IqQJRAk4EAEqwJCJCg1wK0EyJTAtiQQExMYYgtRBxEJUCagAFkPYoJFSpV==


formula: B5
compound: Synthetic
formula_title: <missing>
a: 5.5940
b: 5.5940
c: 12.0756
alpha: 90
beta: 90
gamma: 120
cell_volume: 327.253
crystal_density: 2.469
atoms_sites: ["B1", "B2", "B3", "B4"]
atoms_x: AAAAAKDsCQBwww0AAAAAAA==
atoms_y: AAAAAGAcMwCQRS8AAAAAAA==
atoms_z: gIQeAFAkJwBQoy8AAMslAA==
atoms_occupancy: 0
atoms_u_iso: 4KsAAGBtAAAAfQAA4C4AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High pressure synthesis and investigation of single crystals
 of metastable boron phases
 Note: epsilon-trigonal phase

qdat:
AAAAAAAAAAAAAAAAAAAAAAAIAAgCAAAAAAAAAEAABAAAQCEAEAAAgAAEABABAQAAVABAABACCAFAAAkJABAYAIDAQZAQAQCBDABQIEIDICAAYEBBYECKGgAECCMBgIQAkGABKCBgiEMiAAhEDAgAaCAEoAQQxFCCABAwAQ==


formula: Li
compound: Synthetic
formula_title: <missing>
a: 3.47851
b: 3.47851
c: 3.47851
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.090
crystal_density: 0.548
atoms_sites: ["Li"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Neutron powder-diffraction studies of lithium, sodium and potassium metal
 Note: Body-centered cubic, T = 20 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAAAAQAAAAAAAAAAAABAAAAAAAAAAAQAAAAAAAAAQAAAAAAAAIAAAAAAACAAAAAAAEAAAAAACAAAAAACAAAAAAQAAAAAEAAAAAEAAAAAAAAAABA==


formula: Li
compound: Synthetic
formula_title: <missing>
a: 3.1010
b: 3.1010
c: 22.7649
alpha: 90
beta: 90
gamma: 120
cell_volume: 189.583
crystal_density: 0.547
atoms_sites: ["Li1", "Li2"]
atoms_x: AAAAAAAAAAA=
atoms_y: AAAAAAAAAAA=
atoms_z: AAAAAMCMDQA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Neutron powder-diffraction studies of lithium, sodium and potassium metal
 Note: Hexagonal closest-packed, T = 20 K

qdat:
AAAAAAAAAAAAABAAAAAAAAAAAAACAAAAAAAAAAAIgIAQAIAAAACAACAAAAAAIAAAAAAEAgAAAgAAAAUQQIAAIAIAAAEAAAAAAAAAAAAMBCAAgEAAAgAAAhAAQAAAQAAAAAAAAAAhABAADJEAIIABAAAAAAAAwiAQIACAAA==


formula: Fe7 S8
compound: Synthetic
formula_title: <missing>
a: 11.8656
b: 6.8482
c: 12.8958
alpha: 90
beta: 118.075
gamma: 90
cell_volume: 924.584
crystal_density: 4.651
atoms_sites: ["Fe1", "Fe2", "Fe3", "Fe4", "S1", "S2", "S3", "S4"]
atoms_x: QL0HAACgDwCgCBYAAAAAAKA8NwAgTRUAwB80AKCuJAA=
atoms_y: YEkGAGBDBwAAyggAQBIXACChBwDAsAcAwLAHAOD+BwA=
atoms_z: 4G88ANARDwDwzR4AQEIPAID0NQBA9QYA4HsIAODHJQA=
atoms_occupancy: 0
atoms_u_iso: GLoAABi6AAAYugAAGLoAABi6AAAYugAAGLoAABi6AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structure and magnetism in synthetic pyrrhotite Fe7S8:
 A powder neutron-diffraction study
 Note: T = 11 K

qdat:
AAAAAAAAAAAAAAAAAAIAgAEAAAAAAQEAgiACFAEBgQAACwAhCEIaYCFQBhQKgRVRIDI9AsEOCWAB9gSBoD1HdCAXJZS+1NaXQnJyn2+nWQE1Kzsxbyh9erbvOWKz7vfLjovfzlx+QLs1xKhxksXrd0NRnc96LaqruqPeeZ==


formula: Fe7 S8
compound: Synthetic
formula_title: <missing>
a: 11.9258
b: 6.8822
c: 12.9245
alpha: 90
beta: 118.015
gamma: 90
cell_volume: 936.490
crystal_density: 4.592
atoms_sites: ["Fe1", "Fe2", "Fe3", "Fe4", "S1", "S2", "S3", "S4"]
atoms_x: wLAHAACgDwCg7xUAAAAAAFCrNgAwjRUAEH80AIDEJAA=
atoms_y: 0PwFACC6BwAQjQgAMP4XAMB+BwCwogcAYKcHABCTBwA=
atoms_z: QHk8AOAGDwCAhB4AQEIPALBvNQAgiAcAIGkIAODgJQA=
atoms_occupancy: 0
atoms_u_iso: iJAAAIiQAACIkAAAiJAAAIiQAACIkAAAiJAAAIiQAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structure and magnetism in synthetic pyrrhotite Fe7S8:
 A powder neutron-diffraction study
 Note: T = 298 K

qdat:
AAAAAAAAAAAAAAAAAAYBAAIAAAAAAgEBBEAEKAQDAgAAGgCCEIQlgEUgGCgWBFckgGj0CwQYKcAH1BIFgeU9yQB4nnLblXr9C5tW/Py5yAe6+u+HecNTmdd7lSked9xYpHj846bkBrpafocarG/+tCU33OvDXcrzVD3NsZ==


formula: Pd14 Ag2 Te9
compound: Lukkulaisvaara intrusion, northern Russian Karelia, Russia
formula_title: <missing>
a: 8.9599
b: 8.9599
c: 11.822
alpha: 90
beta: 90
gamma: 90
cell_volume: 949.068
crystal_density: 9.987
atoms_sites: ["PdM1", "PdM2", "PdM3", "AgM4", "Te1", "Te2"]
atoms_x: YOYiADAJKwCAhB4AgIQeAICEHgBgOCYA
atoms_y: YAcRAEDUGAAAAAAAgIQeAICEHgCAeQsA
atoms_z: ABIWAAAAAAAAAAAAcLYLAICEHgCACAkA
atoms_occupancy: 0
atoms_u_iso: mIAAAMB2AABIngAASJ4AAEieAACYigAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Lukkulaisvaaraite, Pd14Ag2Te9, a new mineral from Lukkulaisvaara intrusion,
 northern Russian Karelia, Russia

qdat:
AAAAAAAAAAAAAACAECAAAAAIQAACAoAAAgAIQsAQAgEggBCAElgUKQAyEAiSAwSUSEQIcIVSLJGphgVFiArBtU8w6xxqE0Oxox5S+ErKUNlMVYfjNrYOPtVSMzYsNHN5JRHlxsoCrljEhgk0KSKGGPhABTACAEhUgCEICS==


formula: O
compound: Synthetic
formula_title: <missing>
a: 7.97
b: 5.633
c: 3.711
alpha: 90
beta: 116.3
gamma: 90
cell_volume: 149.359
crystal_density: 2.846
atoms_sites: ["O1", "O2", "O3"]
atoms_x: QGoyAAAjDwCAMgIA
atoms_y: AAAAAAAAAABQShAA
atoms_z: wJ4KAEBaCwAgDAsA
atoms_occupancy: 0
atoms_u_iso: YOoAAMDaAABAGQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 X-ray crystallography of simple molecular solids up to megabar pressures:
 application to solid oxygen and carbon dioxide

qdat:
AAAAAAAAAAAAAAAAAAAAAAACAAAAAIAEAAAAAQAAAAAAIAAJCAACAAAAACCAAAAiAAAgCIAgAQICABAAqAAAAQIAkAkAQUqEAEAAAUBMICAqAFCEgQAZjIIAQIhgABgIlQMoRYYAyNJQAIgYYQSAnKBXyKAiAkC5SPIgI1==


formula: O
compound: Synthetic
pub_title: Structural studies of beta-O2 under pressure
formula_title: <missing>
a: 2.826
b: 2.826
c: 10.160
alpha: 90
beta: 90
gamma: 120
cell_volume: 70.270
crystal_density: 2.268
atoms_sites: ["O"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: YIgDAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAgAAEAAAAAAAAAAAIABAAAAAgAAAAAAQAAAAAIAABAAQAgAAABAAgEAABAAAAAAAAAAADACAgAADAEAAAIAAAIAAAgAwAAAAAQAEAAAAAQAAEAQECAAICEACAAA==


formula: O
compound: Synthetic
pub_title: Structure of 'Orange' 18O2 at 9.6 GPa and 297 K
formula_title: <missing>
a: 4.2151
b: 2.9567
c: 6.6897
alpha: 90
beta: 90
gamma: 90
cell_volume: 83.372
crystal_density: 2.549
atoms_sites: ["O"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: 8FAFAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAAgAACAAAAAAAACAAACBAAAAAABAAAAAAEAAgAAAgAEAAEAAgAkgAAAIAAAAQARAAAQAACAAAHBAAAgAAIgCAASAAARACUgAACABAgAIAQQkYIigEAABACCIQg==


formula: Tl
compound: Synthetic
pub_title: A high-pressure study of thallium Note: Hexagonal closest-packed
formula_title: <missing>
a: 3.463
b: 3.463
c: 5.539
alpha: 90
beta: 90
gamma: 120
cell_volume: 57.526
crystal_density: 11.799
atoms_sites: ["Tl"]
atoms_x: VVgUAA==
atoms_y: q7AoAA==
atoms_z: QEIPAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgABACAAAAAAAAAAAEAAAAAAAAEAAAAACAABAIIAACAAAEAAAIAAAAAAgAIAIABAABBAAgBAAAIAAIAIAAAECIAgAAABBIEQAEQQAABAgCBACACAJAACBIQIEQBEBAgEJAEB==


formula: V S4
compound: Minasraga, Peru
pub_title: Strukturverfeinerung des Patronits, V(S2)2
formula_title: <missing>
a: 6.775
b: 10.42
c: 12.11
alpha: 90
beta: 100.8
gamma: 90
cell_volume: 839.769
crystal_density: 2.835
atoms_sites: ["V1", "S1", "S2", "S3", "S4"]
atoms_x: 4Pz//3CK8f+wkPH/oPQQALA9AwA=
atoms_y: UBQAAED7BQBwIvr/IAoDAIAuCwA=
atoms_z: 0CgHAEBODQBgSw4A4L4BAPA8AAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["V1", "S1", "S2", "S3", "S4"]
atoms_aniso_u11: SIUAAEDEAABYtgAAyJYAAPDcAAA=
atoms_aniso_u22: uG8AAEijAAB4tAAAEL0AAICJAAA=
atoms_aniso_u33: SHsAAGCGAAB4vgAAYIYAAOCcAAA=
atoms_aniso_u12: EPX//3gFAACY7///AAAAAPjp//8=
atoms_aniso_u13: 6CsAAKg+AADoRAAAKDIAAOhEAAA=
atoms_aniso_u23: UOz//9gJAADYCQAAAAAAACj2//8=
qdat:
AAAAAAAAAAAAAAAAACCAQBgAAACCAAAEAQiRAIBCUQIDBAAAYgGkDFIRkBiSYohgDroQ0pG6h8CqGjAYZdJofi8d5uY7vIs2fm9cl6j13uX/LfrF9e8X8VX70bza4/Gmt2uT6C3Ktpo8+tuDroaUG65nk7M+acjhMr740j==


formula: Ca Se O4 H2
compound: Little Eva mine, Grand County, Utah, USA
pub_title: Nestolaite, CaSeO3*H2O, a new mineral from the Little Eva mine, Grand County, Utah, USA
formula_title: <missing>
a: 7.6502
b: 6.7473
c: 7.9358
alpha: 90
beta: 108.542
gamma: 90
cell_volume: 388.368
crystal_density: 3.165
atoms_sites: ["Ca", "Se", "O1", "O2", "O3", "Wat4"]
atoms_x: QPsFAAAjDwAAHRAA4GMMAGDYAwAgTRUA
atoms_y: oNkIAHAIKADACCMAIKwaAMAxMQBgSQYA
atoms_z: QJsVAIAHHgDgqSoA4CEXAIATHADAcyYA
atoms_occupancy: 0
atoms_u_iso: ANwFAOAWBAAgywAAIMsAACDLAADA1AEA
atoms_aniso_label: ["Se"]
atoms_aniso_u11: QIQEAA==
atoms_aniso_u22: YFsDAA==
atoms_aniso_u33: YMwFAA==
atoms_aniso_u12: QAcEAA==
atoms_aniso_u13: gKkDAA==
atoms_aniso_u23: AFkGAA==
qdat:
AAAAAAAAAAAAAAEAAAAABQAAAAABBAAhBAwQAAGgACIIEAgoDACAgIRGAHNBEBkCAGQQkQJKyJTCQonMCkVOJ9GkzwWIhbZXD3qVKlqRxumM3Hy5Vi5W+9zff6s+2jccz+93eTTKo4//fu/++/27+uf//Nv3f/vff7///X==


formula: Fe K Cl3
compound: Synthetic
pub_title: Neutron-diffraction study of the magnetic structure of KFeCl3
formula_title: <missing>
a: 8.715
b: 3.845
c: 14.15
alpha: 90
beta: 90
gamma: 90
cell_volume: 474.155
crystal_density: 2.820
atoms_sites: ["Fe", "K", "Cl1", "Cl2", "Cl3"]
atoms_x: wCEKAOAJGwCgqRAA4G8KAAB3AQA=
atoms_y: QEIPAEBCDwBAQg8AQEIPAEBCDwA=
atoms_z: 4JkDAEBwMQBAVAwA4PcdAGAdNwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAARAAAAgAAAAgQAAQCCAiIAQJwRwAAsAYBjEiAMDA0kSMaMWuJidgGMmCuXKuk+nwpltUs8pucPhz+eVv6h52eX6+rPrWrdY47vf3HI/9mUo+4y9+faja1jvWjhTPt+9V7mXL+SrIz8uhO9vZEkxaC9qtZ==


formula: Fe K Cl3
compound: Synthetic
pub_title: Neutron-diffraction study of the magnetic structure of KFeCl3
formula_title: <missing>
a: 8.715
b: 3.845
c: 14.15
alpha: 90
beta: 90
gamma: 90
cell_volume: 474.155
crystal_density: 2.820
atoms_sites: ["Fe", "K", "Cl1", "Cl2", "Cl3"]
atoms_x: AEEKAADhGQDgSxAAQOMJAGDqAAA=
atoms_y: QEIPAEBCDwBAQg8AQEIPAEBCDwA=
atoms_z: IDwDAEDtMQAAsgwAIBceAEDPNgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAARAAAAgAAAAgQAAQCCAiIAQJwRwAAsAYBjEiAMDA0kSMaEWuJidgGMmCuXKuk+nwpltUs8pucPhz+eVv6h52cX6+rPrWrdY47vf3HI/9mUo+4y9+faja1jvWjhSPt+9V7mXL+SrIz8uhO9vZEkxaC9qtZ==


formula: K Fe Cl3
compound: Synthetic
pub_title: Preparation and crystal structure of KFeCl3 and KFeBr3
formula_title: <missing>
a: 8.712
b: 3.845
c: 14.15
alpha: 90
beta: 90
gamma: 90
cell_volume: 473.992
crystal_density: 2.821
atoms_sites: ["K", "Fe", "Cl1", "Cl2", "Cl3"]
atoms_x: wLsaAOBvCgCgLBAAQGAKAIC7AAA=
atoms_y: QEIPAEBCDwBAQg8AQEIPAEBCDwA=
atoms_z: oFoyAOAcAwBATg0AAEYeAAAtNwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAARAAAAAAAAAgQAAQCCAiIAQJwRwAAsAYBjEiAMDA0kJMYMVuJidgFMiCuXK+i+n4lltUs8o+cPh7+eTvah52eX6+rPrWq1Y07vf3nI/9mUo+4q9+Lfjazju3jhJPdv9V7mWreS7Iz8thOtvZEkxZC76tZ==


formula: K Fe Br3
compound: Synthetic
pub_title: Preparation and crystal structure of KFeCl3 and KFeBr3
formula_title: KFeBr3
a: 8.712
b: 3.845
c: 14.15
alpha: 90
beta: 90
gamma: 90
cell_volume: 473.992
crystal_density: 4.690
atoms_sites: ["K", "Fe", "Br1", "Br2", "Br3"]
atoms_x: IJodAOD4CAAg6BAAQFoLAKCAAgA=
atoms_y: QEIPAEBCDwBAQg8AQEIPAEBCDwA=
atoms_z: 4Oo0ACC5AwDg5gsAgAEfAAC2NQA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAARAAAAgAAAAgQAAQCCAiIAQJwRwAAsAYBjEiAMDA0kJMaMVuJidgFMiCuXK+i+n4lltUs8o+cPh7+eTvah52eX6+rPrWq1Y07vf3nI/9mUo+4q9+Lfjazju3jhJPdv9V7mWreS7Iz8thOtvZEkxZC76tZ==


formula: As S
compound: Fergana Valley, Alai Range, Osh Oblast, Kyrgyzstan
formula_title: <missing>
a: 9.956
b: 9.308
c: 8.869
alpha: 90
beta: 102.55
gamma: 90
cell_volume: 802.257
crystal_density: 3.543
atoms_sites: ["As1", "As2", "S1", "S2", "S3"]
atoms_x: oOL//5A49v8AAAAAAAAAAEC48/8=
atoms_y: 2HXz/1B95//ASwMAAMohAABy7f8=
atoms_z: +FkDAHiyBwBAQg8AQEIPADDFFAA=
atoms_occupancy: 0
atoms_u_iso: AMIBADC6AQCQDgIAgDICAMAfAgA=
atoms_aniso_label: ["As1", "As2", "S1", "S2", "S3"]
atoms_aniso_u11: UCECAFByAQDguAIAoDUCADChAQA=
atoms_aniso_u22: 0BQCAHDyAQAgYQEA4FoBAOADAwA=
atoms_aniso_u33: cBEBAKCGAQAADQIAsKcCANDiAQA=
atoms_aniso_u12: 8FUAANAHAAAAAAAAAAAAAEC7//8=
atoms_aniso_u13: MFwAAKDE//9wewAAILj//2C4AAA=
atoms_aniso_u23: sGgAAHCa//8AAAAAAAAAAACc//8=
pub_title:
 From ancient pigments to modern optoelectronic applications of arsenic sulfides:
 bonazziite, the natural analogue of beta-As4S4 from Khaidarkan deposit, Kyrgyzstan

qdat:
AAAAAAAAAAAAAAAEAAAAAUEAQEAAAACQAgQaAAUAACSQQhCAKBgYMpBhAdJgAJIcPQhMEgRGyBAo+TBFiDrxF5egJgnT8ctVz6Kd5bXmT1+2N89eU632/Dyrv02/63f+dt0W/r15n4dx5ps7+ffDE9lEGvHr0kgNJ5MitT==


formula: Cu3.99 Br.95 Cl.09 F O5.85 H5.85
compound: Great Australia mine, Cloncurry, Queensland, Australia
formula_title: <missing>
a: 6.6786
b: 6.6786
c: 9.2744
alpha: 90
beta: 90
gamma: 120
cell_volume: 358.251
crystal_density: 4.182
atoms_sites: ["Cu1", "Cu2", "Br", "Cl", "F", "O", "H"]
atoms_x: gIQeAPilFgCrsCgAq7AoAAAAAACIUgwAEHoHAA==
atoms_y: AAAAAFBLLQBVWBQAVVgUAAAAAAB4tjAA8I41AA==
atoms_z: AAAAAMDGLQDAxi0AwMYtAMDGLQAIazcAYCk1AA==
atoms_occupancy: AAk9AEAkFADA+zkAQH4FAAAJPQBggjsAYII7AA==
atoms_u_iso: aOIAADDAAACAHwEAgB8BAKCGAQBQwwAAgK8CAA==
atoms_aniso_label: ["Cu1", "Cu2", "Br", "Cl", "F", "O"]
atoms_aniso_u11: QKYAAJCwAAAQOgEAEDoBAEBLAQDAqAAA
atoms_aniso_u22: QJwAALAXAQAQOgEAEDoBAEBLAQDAqAAA
atoms_aniso_u33: IGEBACCZAADw6wAA8OsAAKADAgBw+AAA
atoms_aniso_u12: 0E0AAKCMAAC4nAAAuJwAAKClAABgVAAA
atoms_aniso_u13: KOL//wAAAAAAAAAAAAAAAAAAAADw8f//
atoms_aniso_u23: UMT//wAAAAAAAAAAAAAAAAAAAAAQDgAA
pub_title:
 Barlowite, Cu4FBr(OH)6, a new mineral isostructural with claringbullite:
 description and crystal structure

qdat:
AAAAAAAAAAAAAAAAAAQAAIEAAAAAAgAIAAAAQAqAAACAAQABCUAAAgIkABDIAACAgJShAgSAIMiBBIJJggQiAJpAACMxcIkDGoEQJWUYoIqRCQ22NTMdgamoxGKFRMJ1yYM3EIdMiR1CRJUSzMCz2ZCKyAGmbD/FA8lZ2l==


formula: Ca Na3 Al Mg3 F14
compound: Cleveland tin mine, Luina, western Tasmania
formula_title: <missing>
a: 7.1756
b: 7.1756
c: 7.1756
alpha: 59.867
beta: 59.867
gamma: 59.867
cell_volume: 260.464
crystal_density: 3.028
atoms_sites: ["Ca", "Na", "Al", "Mg", "F1", "F2", "F3"]
atoms_x: AAAAAICEHgCAhB4AgIQeAOBvCgCwrRoA4JoHAA==
atoms_y: AAAAAAAAAACAhB4AgIQeAOBvCgCwrRoA4JoHAA==
atoms_z: AAAAAAAAAACAhB4AAAAAACBEIwDw3jAA4JoHAA==
atoms_occupancy: 0
atoms_u_iso: kMkAACAvAQBAagAAsGgAAGC4AADAwQAA0LYAAA==
atoms_aniso_label: ["Ca", "Na", "Al", "Mg", "F1", "F2", "F3"]
atoms_aniso_u11: ENYAACCZAADwbgAAQGoAAOCSAACg8AAAQLUAAA==
atoms_aniso_u22: ENYAADCIAQDwbgAAQGoAAOCSAACg8AAAQLUAAA==
atoms_aniso_u33: ENYAADCIAQDwbgAAgFcAAJDiAABghgAAQLUAAA==
atoms_aniso_u12: ULD//xDD//9g1///ENz//6D2//8Qqv//oMT//w==
atoms_aniso_u13: ULD//xDD//9g1///cOX//7C5//+wuf//oMT//w==
atoms_aniso_u23: ULD//6Au//9g1///cOX//7C5//+wuf//oMT//w==
pub_title:
 Coulsellite, CaNa3AlMg3F14, a rhombohedral pyrochlore with 1:3 ordering
 in both A and B sites, from the Cleveland mine, Tasmania, Australia

qdat:
AAAAAAAAAAAAAAAAAAAACAAAAAAAAQAAAAYAAAAAAIAAAgQAAAAAAGAAAAIAAwgAAIADEAAAAAIAAYAYAACAEwAEABgAIAwACgEAAADYAYDUAAC4AAAACA4AcDwAgCAYOACD4ABsBR8Aw4AAKBwwBD4FAAMOAQeAC4GOAQ==


formula: La F3
compound: Synthetic
formula_title: <missing>
a: 7.185
b: 7.185
c: 7.351
alpha: 90
beta: 90
gamma: 120
cell_volume: 328.648
crystal_density: 5.939
atoms_sites: ["La", "F1", "F2", "F3"]
atoms_x: YEUoADBVFgBVWBQAAAAAAA==
atoms_y: AAAAAIBFAwCrsCgAAAAAAA==
atoms_z: QEIPAFD2BACwWAsAQEIPAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["La", "F1", "F2", "F3"]
atoms_aniso_u11: yFUAAEBaAQBQbgAAoH0AAA==
atoms_aniso_u22: yFUAAPDrAABQbgAAoH0AAA==
atoms_aniso_u33: CE0AAOCIAACQPAEAwHQCAA==
atoms_aniso_u12: +CoAAFjKAAAoNwAAYEAAAA==
atoms_aniso_u13: MAcAAND4//8AAAAAAAAAAA==
atoms_aniso_u23: 8AoAAFjf//8AAAAAAAAAAA==
pub_title:
 Refinement of the trigonal structure of lanthanum trifluoride
 with neutron diffraction data
 Note: neutron data

qdat:
AAAAAAAAAAAAAAAABAAAAAAAAAAAEQAAESAAAAAABAAAUACAAAECBAAAAgoIiCIAhAQoAAAAIYSAQwGAAEQIxEAURgYBhGBBIBBIAiItJiwAByIoCEgUiXLEgYYFSIhhiRRMYKWODDUUDDE2O2eOGWoVRZbiVkDEsVxwln==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.394
b: 8.394
c: 8.394
alpha: 90
beta: 90
gamma: 90
cell_volume: 591.435
crystal_density: 5.201
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwDQjg8A
atoms_y: gIQeACChBwDQjg8A
atoms_z: gIQeACChBwDQjg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 0.0001 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAIAAAAAIAAAAAAABAAAAIAAAAAAQAABAAAAAEAABAAAABAABAAAAEAAgAAAIABAAABAAQAABAAgAACACAAAgAgAAIAQAAQAgAAACAACAIAAQBAAEAQACAIABAIAAAQACAQAA==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.350
b: 8.350
c: 8.350
alpha: 90
beta: 90
gamma: 90
cell_volume: 582.183
crystal_density: 5.283
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwCglg8A
atoms_y: gIQeACChBwCglg8A
atoms_z: gIQeACChBwCglg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 2.9 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAEAAAAACAAAAAAAAQAAACAAAAAAEAAAQAAAAAgAAQAAAAIAAQAAABAAEAAABAAIAAAIACAAAEACAAAQAIAACACAABABAABABAAAAEAAIAgAAgEAAQBAAEAgAEAQAAAQAEAgA==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.328
b: 8.328
c: 8.328
alpha: 90
beta: 90
gamma: 90
cell_volume: 577.593
crystal_density: 5.325
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwDwkQ8A
atoms_y: gIQeACChBwDwkQ8A
atoms_z: gIQeACChBwDwkQ8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 4.4 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAEAAAAACAAAAAAAAIAAABAAAAAACAAAIAAAAAQAAIAAAAEAAEAAAAQABAAAAgACAAACAAgAACAAgAAEAEAAAgAgAAQAQAAIAgAAABAABAEAAIBAACAIABAEAAgEAAAEAAgEA==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.304
b: 8.304
c: 8.304
alpha: 90
beta: 90
gamma: 90
cell_volume: 572.614
crystal_density: 5.372
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwCwiw8A
atoms_y: gIQeACChBwCwiw8A
atoms_z: gIQeACChBwCwiw8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 6.3 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAACAAAAABAAAAAAAAEAAAAgAAAAABAAAEAAAAAIAACAAAABAACAAAAIAAgAAAIABAAABAAIAAAgAQAABABAAAIAIAAEAEAAEAEAAAAIAAQBAACAIAAgCAAIBAAEAgAAAgAIBA==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.272
b: 8.272
c: 8.272
alpha: 90
beta: 90
gamma: 90
cell_volume: 566.020
crystal_density: 5.434
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwAwmA8A
atoms_y: gIQeACChBwAwmA8A
atoms_z: gIQeACChBwAwmA8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 8.6 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAABAAAAAAgAAAAAAACAAAAQAAAAAAgAABAAAAACAABAAAAAgAAgAAACAAEAAACAAIAAAIACAAAEACAAAQAIAACABAAAgAgAAQAgAAABAACAIAAQAgACAQAAgEAAQEAAACAAgE==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.261
b: 8.261
c: 8.261
alpha: 90
beta: 90
gamma: 90
cell_volume: 563.765
crystal_density: 5.456
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwBgkA8A
atoms_y: gIQeACChBwBgkA8A
atoms_z: gIQeACChBwBgkA8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 10.0 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAABAAAAAAgAAAAAAACAAAAQAAAAAAQAABAAAAACAAAgAAAAQAAQAAABAAEAAABAAIAAAEABAAAEABAAAIAEAAAgBAAAQAQAAIAQAAAAgABACAAIAgABAEAAgCAAQBAAABAAIB==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.249
b: 8.249
c: 8.249
alpha: 90
beta: 90
gamma: 90
cell_volume: 561.311
crystal_density: 5.480
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwAQlQ8A
atoms_y: gIQeACChBwAQlQ8A
atoms_z: gIQeACChBwAQlQ8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 11.0 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAABAAAAAAQAAAAAAABAAAAIAAAAAAQAAAgAAAABAAAQAAAAIAAIAAAAgACAAAAgAEAAAEABAAACAAgAAEACAAAgAQAAIAIAAEAIAAAAQAAgBAACAIAAgCAAIBAAEAgAAAQAEA==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.236
b: 8.236
c: 8.236
alpha: 90
beta: 90
gamma: 90
cell_volume: 558.662
crystal_density: 5.506
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwCglg8A
atoms_y: gIQeACChBwCglg8A
atoms_z: gIQeACChBwCglg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 12.1 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAgAAAAAQAAAAAAABAAAAEAAAAAAIAAAgAAAAAgAAQAAAAIAAIAAAAQABAAAAQACAAACAAQAABAAQAACABAAAIAIAACAEAACAEAAAAIAAIAgABAEAAIBAACAQABAIAAAIABA==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.225
b: 8.225
c: 8.225
alpha: 90
beta: 90
gamma: 90
cell_volume: 556.427
crystal_density: 5.528
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwCglg8A
atoms_y: gIQeACChBwCglg8A
atoms_z: gIQeACChBwCglg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 12.9 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAgAAAAAQAAAAAAABAAAAEAAAAAAIAAAQAAAAAgAAIAAAAEAAEAAAAQAAgAAAQABAAABAAQAAAgAIAABAAgAAEAEAACACAABACAAAACAAEAQAAgCAAEAQACAEAAgEAAAEAAg==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.207
b: 8.207
c: 8.207
alpha: 90
beta: 90
gamma: 90
cell_volume: 552.781
crystal_density: 5.564
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwCAkw8A
atoms_y: gIQeACChBwCAkw8A
atoms_z: gIQeACChBwCAkw8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 14.4 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAQAAAAAIAAAAAAAAgAAACAAAAAAEAAAIAAAAAQAAEAAAACAACAAAAIAAQAAAEAAgAAAgAEAAAIAEAAAQAIAACACAAAgAgAAQAgAAABAACAEAAIAQABAIAAQCAAIBAAABAAI==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.198
b: 8.198
c: 8.198
alpha: 90
beta: 90
gamma: 90
cell_volume: 550.965
crystal_density: 5.583
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwCglg8A
atoms_y: gIQeACChBwCglg8A
atoms_z: gIQeACChBwCglg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 15.1 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAQAAAAAIAAAAAAAAQAAACAAAAAAEAAAIAAAAAIAACAAAABAABAAAAEAAQAAAEAAQAAAQAEAAAIACAAAIAIAABABAAAQAgAAIAQAAAAgAAgCAAEAQAAgCAAIBAAEAgAAAgAC==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.184
b: 8.184
c: 8.184
alpha: 90
beta: 90
gamma: 90
cell_volume: 548.147
crystal_density: 5.611
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwDwkQ8A
atoms_y: gIQeACChBwDwkQ8A
atoms_z: gIQeACChBwDwkQ8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 16.0 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAQAAAAAEAAAAAAAAQAAABAAAAAACAAAEAAAAAIAACAAAAAgAAgAAACAAIAAABAAIAAAIABAAACABAAAEACAAAgAgAAIAIAAEAIAAAAQAAQAgABAEAAQBAAEAgABAQAAAIAB==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.174
b: 8.174
c: 8.174
alpha: 90
beta: 90
gamma: 90
cell_volume: 546.140
crystal_density: 5.632
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwBwhQ8A
atoms_y: gIQeACChBwBwhQ8A
atoms_z: gIQeACChBwBwhQ8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 17.0 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAQAAAAAEAAAAAAAAQAAABAAAAAABAAAEAAAAAEAABAAAAAgAAgAAACAAEAAABAAEAAAEABAAACAAgAAEACAAAQAQAAEAEAACAEAAAAIAAIAgAAgCAAIAgABAIAAgEAAAEAA==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.158
b: 8.158
c: 8.158
alpha: 90
beta: 90
gamma: 90
cell_volume: 542.939
crystal_density: 5.665
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwCwiw8A
atoms_y: gIQeACChBwCwiw8A
atoms_z: gIQeACChBwCwiw8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 18.1 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAAAgAAAAABAAACAAAAACAABAAAAAQAAQAAAAgACAAAAgAEAAACAAgAAAgAQAABAAgAAEAEAABACAAAgBAAAACAACAIAAQBAACAIAAgCAAQBAAAAgA==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.149
b: 8.149
c: 8.149
alpha: 90
beta: 90
gamma: 90
cell_volume: 541.144
crystal_density: 5.684
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwBAjQ8A
atoms_y: gIQeACChBwBAjQ8A
atoms_z: gIQeACChBwBAjQ8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 19.1 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAQAAQAAAAgABAAAAQACAAABAAQAAAgAIAABAAgAAEACAABABAAAgAgAAABAABAEAAEAQABAEAAQBAAEAgAAAgA==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.138
b: 8.138
c: 8.138
alpha: 90
beta: 90
gamma: 90
cell_volume: 538.956
crystal_density: 5.707
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwBwhQ8A
atoms_y: gIQeACChBwBwhQ8A
atoms_z: gIQeACChBwBwhQ8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 20.0 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAEAAAAQAAAAAAgAABAAAAABAAAQAAAAIAAIAAAAQAAgAAAIABAAAAgAIAAAQAEAAAQAIAACACAAAQAgAAQAQAAAAgAAgCAAEAIAAQCAAEAgACAQAAAIA==


formula: Fe3 O4
compound: Synthetic
formula_title: <missing>
a: 8.125
b: 8.125
c: 8.125
alpha: 90
beta: 90
gamma: 90
cell_volume: 536.377
crystal_density: 5.734
atoms_sites: ["Fe1", "Fe2", "O"]
atoms_x: gIQeACChBwDggw8A
atoms_y: gIQeACChBwDggw8A
atoms_z: gIQeACChBwDggw8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effect of high pressure on the crystal structure and electronic properties
 of magnetite below 25 GPa
 Note: P = 21.1 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAACAAAAAAAAEAAAAQAAAAAAQAAAgAAAABAAAQAAAAEAAEAAAAIAAgAAAEAAgAAAQAEAAAIACAAAIAEAABAAgAAIAIAAEAIAAAAQAAQAgABAEAAIAgACAQABAIAAAEA==


formula: Zn2 As O5 H
compound: Ojuela Mine, Mapimi, Durango, Mexico
formula_title: <missing>
a: 5.8438
b: 6.7226
c: 5.6566
alpha: 104.348
beta: 92.320
gamma: 76.683
cell_volume: 209.470
crystal_density: 4.546
atoms_sites: ["Zn1", "Zn2", "As", "O1", "O2", "O3", "O4", "O5", "H"]
atoms_x: sMwtALgjEACw6i0A4NcBAEA7JQAAsiUAgGEPAICXBgBgSQYA
atoms_y: cI8eADhnCwCQwxAAEI0IAACeBwAQXhQA0GYeABBREgDAmAsA
atoms_z: 8PwXABBJAQBwvDIA0IMuAACFOQBwWCMAEEI6AFB3FQDAxxgA
atoms_occupancy: 0
atoms_u_iso: 0NQAAIi9AAAwiQAAsMwAAKDXAADQzwAAUKoAAADIAADgKAEA
atoms_aniso_label: ["Zn1", "Zn2", "As", "O1", "O2", "O3", "O4", "O5"]
atoms_aniso_u11: YLgAAIiGAACwbQAA8IcAACCAAAAArwAAMKcAAMDaAAA=
atoms_aniso_u22: YBwBABDWAAA4lQAAMAsBAPC5AADQMwEAMI4AAACvAAA=
atoms_aniso_u33: SK0AACjSAACAmAAAoL4AAIBqAQCAogAAYLgAAGDRAAA=
atoms_aniso_u12: YNf//wDx//9A8v//QO3///AKAAAQw///0O7//4Da//8=
atoms_aniso_u13: SBIAAIgdAABoGgAAUBQAANA5AACwHQAAQB8AAEA4AAA=
atoms_aniso_u23: yEYAAAAyAAC4LgAAECcAAECcAACAVwAAUBQAAJAzAAA=
pub_title:
 Crystal structure refinements of legrandite, adamite, and paradamite:
 The complex structure and characteristic hydrogen bonding network of legrandite

qdat:
AAAAAAAAAAAAAAAAEAEQABAAAAIAQAAIAggABAQAAQykAQAQBEEACAiUOMQBAEDEKIiFBCBWB2ChECJAIxWj0QwxIxEEsH4E08dQbVBnBcBDnWvvfqGdedi3oKy3mv1Th8vu5/V1YzzZ395XPv5f+by/9bX+/Tv9Hvz75z==


formula: Zn2 As O5 H
compound: Ojuela Mine, Mapimi, Durango, Mexico
formula_title: <missing>
a: 8.3428
b: 8.5664
c: 6.0769
alpha: 90
beta: 90
gamma: 90
cell_volume: 434.302
crystal_density: 4.385
atoms_sites: ["Zn1", "Zn2", "As", "O1", "O2", "O3", "O4", "H"]
atoms_x: AAAAABA9CAAYTA8A4JMEACCOBgAgIhgAEHYQAKBEDAA=
atoms_y: AAAAAGg7FgDI4g4AYNMIAJDRBwAgXAYAMAoWAADcBQA=
atoms_z: GBoPAAAAAACAhB4AgIQeAAAAAACAhB4AQOsQAAAAAAA=
atoms_occupancy: 0
atoms_u_iso: cN8AAGCfAABQeAAAQJwAAECcAACg8AAAcN8AAGDqAAA=
atoms_aniso_label: ["Zn1", "Zn2", "As", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: oDsBAMCoAACQfgAA4KsAAECcAACgjAAAwPMAAA==
atoms_aniso_u22: QOcAAMCPAABAagAAYG0AAGBtAABgbQAAQBkBAA==
atoms_aniso_u33: 4HkAADCnAACwgQAAIMsAACDLAADA1AEAwI8AAA==
atoms_aniso_u12: kJ3//8D5//8AAAAA0KP//xAOAACw6///ULD//w==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAoMT//w==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAsDYAAA==
pub_title:
 Crystal structure refinements of legrandite, adamite, and paradamite:
 The complex structure and characteristic hydrogen bonding network of legrandite

qdat:
AAAAAAAAAAAAAAAAAEAAAYAAEQAEgAAAFAEgAADkEIKQtAAChQUDEYGpSCFBBSdMnywIckSZabeOYMQWlo9D1Me63dNYV23+e9sX/2/uF6/8O9qv/79958ju/9//73/7+/f9X/P/7982/7/+fvbPX/9+zrfnX/z7//T91T==


formula: C H4 N2 O
compound: Synthetic
formula_title: <missing>
a: 5.584
b: 5.584
c: 4.689
alpha: 90
beta: 90
gamma: 90
cell_volume: 146.208
crystal_density: 1.364
atoms_sites: ["C", "H1", "H2", "N", "O"]
atoms_x: AAAAAFCbDwDwuwgA8NQIAAAAAAA=
atoms_y: gIQeANAfLgBwQCcAcFknAICEHgA=
atoms_z: AAUUABBXEQBA4P3/EOUKAKBjJAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["C", "H1", "H2", "N", "O"]
atoms_aniso_u11: sOUAAICvAgDgnwIA4L4BANAzAQA=
atoms_aniso_u22: sOUAAICvAgDgnwIA4L4BANAzAQA=
atoms_aniso_u33: kGUAAIBRAQDA2gAAcJQAAHBiAAA=
atoms_aniso_u12: kAEAACCl/v8gCf//UBr//5AaAAA=
atoms_aniso_u13: AAAAAJDP//+wHQAAIAMAAAAAAAA=
atoms_aniso_u23: AAAAAJDP//+wHQAAIAMAAAAAAAA=
pub_title:
 The crystal structure and molecular thermal motion of urea
 at 12, 60 and 123 K from neutron diffraction
 Note: neutron data, T = 123 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAEAAAAAAACAAEAAAAgCCAAEAAAAggAAAEIIAIAIAAAiAIAQgAQgBIIkEgCBAEBIAMAIASAyFASACgIFgEgYIIICkAjQSBSKiQUCAFFBYEFgKElJSUKSoQFCUhEgUC1ShUqBcDmTLrRUsY==


formula: C H4 N2 O
compound: Synthetic
formula_title: <missing>
a: 5.570
b: 5.570
c: 4.688
alpha: 90
beta: 90
gamma: 90
cell_volume: 145.445
crystal_density: 1.371
atoms_sites: ["C", "H1", "H2", "N", "O"]
atoms_x: AAAAABCuDwDgxggAcOEIAAAAAAA=
atoms_y: gIQeAJAyLgBgSycA8GUnAICEHgA=
atoms_z: kO0TAABJEQBQvP3/MM8KACBXJAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["C", "H1", "H2", "N", "O"]
atoms_aniso_u11: gIkAAND7AQAwBQIA8AQBABC9AAA=
atoms_aniso_u22: cEkAAND7AQAwBQIA8AQBAPA8AAA=
atoms_aniso_u33: cEkAAEAyAQCgvgAA0GsAAPA8AAA=
atoms_aniso_u12: cP7//2D2/v9AV///wHz//5ABAAA=
atoms_aniso_u13: AAAAAPDY///QIAAAsAQAAAAAAAA=
atoms_aniso_u23: AAAAAPDY///QIAAAsAQAAAAAAAA=
pub_title:
 The crystal structure and molecular thermal motion of urea
 at 12, 60 and 123 K from neutron diffraction
 Note: neutron data, T = 60 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAACAAAAAAACAACAAAAgCCAACAAAAgQAAACIEAIAEAAAhAEAIgAIQBEERCQBAgEAkAMAIAQgZCgFACQECwBIMCCCDRAJsFhJJIsHCACUgsCCwEhjknZCxUIDRQwjQHB5UoOVgvAyFTu4aTT==


formula: C H4 N2 O
compound: Synthetic
formula_title: <missing>
a: 5.565
b: 5.565
c: 4.684
alpha: 90
beta: 90
gamma: 90
cell_volume: 145.060
crystal_density: 1.375
atoms_sites: ["C", "H1", "H2", "N", "O"]
atoms_x: AAAAAHC3DwCQywgAsOcIAAAAAAA=
atoms_y: gIQeAPA7LgAQUCcAMGwnAICEHgA=
atoms_z: wOUTADBBEQBArv3/YMcKAJBVJAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["C", "H1", "H2", "N", "O"]
atoms_aniso_u11: cGIAANCwAQBgywEAkLAAAPCHAAA=
atoms_aniso_u22: cGIAANCwAQBgywEAkLAAAPCHAAA=
atoms_aniso_u33: sDYAABAhAQBAtQAAMFwAAAAyAAA=
atoms_aniso_u12: IAMAAJAg//8gbf//wK7//yADAAA=
atoms_aniso_u13: AAAAALDS//9wFwAAQAYAAAAAAAA=
atoms_aniso_u23: AAAAALDS//9wFwAAQAYAAAAAAAA=
pub_title:
 The crystal structure and molecular thermal motion of urea
 at 12, 60 and 123 K from neutron diffraction
 Note: neutron data, T = 12 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAACAAAAAAABAACAAAAQBCAACAAAAgQAAACEEAIAEAAAhAEAEQAIIBCERCQBAQCAkAGAEAIgIigFABIEB4BEGBCCBxAFUDgkFEUFBABSQUBBYChRSitBoqEBo4oSoDg9KULKwXgbCp3cNJp==


formula: (Ni1.05 Co1.95) P2 O8
compound: Synthetic
formula_title: (Ni0.35Co0.65)3(PO4)2
a: 10.247
b: 4.728
c: 5.889
alpha: 90
beta: 91.07
gamma: 90
cell_volume: 285.259
crystal_density: 4.267
atoms_sites: ["NiM1", "CoM1", "NiM2", "CoM2", "P", "O1", "O2", "O3", "O4"]
atoms_x: AAAAAAAAAADgyBAA4MgQACCtBQCgaAYA4AMcAODsCgCAAgoA
atoms_y: AAAAAAAAAAAg0f//INH//yCyGQBAiC0AALgLAEAqEwBgihAA
atoms_z: gIQeAICEHgDg1A4A4NQOAGCQDwDAehAAYJAPAGBbAwAAzxwA
atoms_occupancy: gBMcAID1IABgARIAoAcrAAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: SJ4AAEieAABIngAASJ4AAGA7AAA4TwAAOE8AADhPAAA4TwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystallographic studies of olivine-related sarcopside-type solid solutions
 Note: neutron data, sample (Ni0.35Co0.65)3(PO4)2

qdat:
AAAAAAAAAAQAAAAAAAAAEAAAIAAAIAaAAAAUARAABJgIIEFKBAgQoBCCBBBgKKBgBRCLBOYdiQNORLoAUjCFWzrBKTNruzLkSbhf9j8F+KaWzuE7WXx35e5elShdZe8+kXCnX/Vqf3vwdW/z1/elfyL1vL9e/2mXMP7Yut==


formula: (Ni2.1 Mn.9) P2 O8
compound: Synthetic
formula_title: (Ni0.70Mn0.30)3(PO4)2
a: 10.267
b: 4.726
c: 5.961
alpha: 90
beta: 90.82
gamma: 90
cell_volume: 289.209
crystal_density: 4.164
atoms_sites: ["NiM1", "MnM1", "NiM2", "MnM2", "P", "O1", "O2", "O3", "O4"]
atoms_x: AAAAAAAAAABgBxEAYAcRAGDMBQDgCgYA4AMcAEBgCgCg0wkA
atoms_y: AAAAAAAAAACgFf//oBX//8DBGQBg1i0AQNcLAACOEgCAWxAA
atoms_z: gIQeAICEHgCgtQ4AoLUOAODODwBgihAA4M4PAADoAwBgvxwA
atoms_occupancy: gO42AIAaBgAAnyQAAGoYAAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: KOz//yjs//8o7P//KOz//9gTAAA4TwAAOE8AADhPAAA4TwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystallographic studies of olivine-related sarcopside-type solid solutions
 Note: neutron data, sample (Ni0.70Mn0.30)3(PO4)2

qdat:
AAAAAAAAAAQAAAAAAAAAIAAAIAAAIASAAAAwCBAABFBAIEEiBBAhgBQCFUWAIwIgEQQODGy1gWOalxgA4NAjvHyEDYe9zzGMuOp7LRobsoxrNRyYbfr6e12tNCraH/HSz1qXu4XemPVl99N3905NE/Lthuc3+1j7/W/t//==


formula: (Ni1.95 Co1.05) P2 O8
compound: Synthetic
formula_title: (Ni0.65Co0.35)3(PO4)2
a: 10.185
b: 4.713
c: 5.865
alpha: 90
beta: 91.09
gamma: 90
cell_volume: 281.480
crystal_density: 4.321
atoms_sites: ["NiM1", "CoM1", "NiM2", "CoM2", "P", "O1", "O2", "O3", "O4"]
atoms_x: AAAAAAAAAABgBxEAYAcRAGBPBQCAGgYAQPQbAAC+CgCAhQkA
atoms_y: AAAAAAAAAABAov//QKL//4AfGgDAxi0AQNcLAKAaEwCgqRAA
atoms_z: gIQeAICEHgCA5A4AgOQOAMCADwAg6BAAIO4PAEANAwBgQhwA
atoms_occupancy: gCotAIDeDwAg7SQA4BsYAAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: CBUBAAgVAQAIFQEACBUBAJiKAAAgsgAAILIAACCyAAAgsgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystallographic studies of olivine-related sarcopside-type solid solutions
 Note: neutron data, sample (Ni0.65Co0.35)3(PO4)2

qdat:
AAAAAAAAAAIAAAAAAAAAEAAAEAAAEANAAAAKAIgAAUoEECCTAgIEUAQggwgoFDAYASQkojGH5EDKkS8AEtIQ1crYREbdt2qdET4L/EbBNR0zUtwm0isOrT2q1SeN2y/r8h4Sar3Er/5WBuV+ee/eVfQuj5Plvf2a4w3blp==


formula: Pd2 Si
compound: Synthetic
pub_title: Some notes on the palladium-silicon system
formula_title: <missing>
a: 6.496
b: 6.496
c: 3.433
alpha: 90
beta: 90
gamma: 120
cell_volume: 125.457
crystal_density: 9.567
atoms_sites: ["Pd1", "Pd2", "Si1", "Si2"]
atoms_x: wBYQAOD/JABVWBQAAAAAAA==
atoms_y: AAAAAAAAAACrsCgAAAAAAA==
atoms_z: AAAAAICEHgAAAAAAgIQeAA==
atoms_occupancy: 0
atoms_u_iso: KFUAAEioAACgggAASP0AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAACAAAAAAAAAAAEAQAACAQAAAAAAIAAAQIAAAAABAAgAAgADEAAQAgAMACEAAAIAEQCAAICACACEAYAAKhFAAEATBAAQgAAKgUIBIIgAQAoEARQMCgMMERUAECoQEACjIEEJFgBAuOALBigxYw8Age==


